High temperature superconducting materials

ABSTRACT

A superconducting composition of matter including overlapping first and second regions. The regions comprise unit cells of a solid, the first region comprises an electrical insulator or semiconductor, and the second region comprises a metallic electrical conductor. The second region extends through the solid and a subset of said second region comprise surface metal unit cells that are adjacent to at least one unit cell from the first region. The ratio of the number of said surface metal unit cells to the total number of unit cells in the second region being at least 20 percent.

CROSS REFERENCE TO RELATED APPLICATIONS

This application is a continuation under 35 U.S.C § 120 of U.S. Utility patent application Ser. No. 15/896,697, filed on Feb. 14, 2018, entitled “HIGH TEMPERATURE SUPERCONDUCTING MATERIAL” by Jamil Tahir-Kheli, which application claims the benefit under 35 U.S.C. Section 119(e) of co-pending and commonly-assigned U.S. Provisional Patent Application Ser. No. 62/458,740, filed on Feb. 14, 2017, by Jamil Tahir-Kheli, entitled “HIGH TEMPERATURE SUPERCONDUCTING MATERIALS,” CIT-7708); both of which applications are incorporated by reference herein.

STATEMENT REGARDING GOVERNMENT SUPPORT

This invention was made with government support under Grant No, N00014-18-1-2679 awarded by the Office of Naval Research. The government has certain rights in the invention.

BACKGROUND OF THE INVENTION 1. Field of the Invention

The present invention relates to superconducting materials and methods of fabricating the same.

2. Description of the Related Art

(Note: This application references a number of different publications as indicated throughout the specification by one or more reference numbers in brackets, e.g., [x]. A list of these different publications ordered according to these reference numbers can be found below in the section entitled “References.” Each of these publications is incorporated by reference herein.)

The cuprate superconductors were discovered experimentally by materials scientists in 1986. Since then, there have been over 200,000 refereed papers on cuprate superconductivity, yet the mechanism that leads to superconductivity is unknown. It has been 24 years since the last discovery of the highest temperature superconductor at ambient pressure with a superconducting transition temperature, Tc, of 139 Kelvin. In addition, the critical current density, Jc, is 100 times smaller than the theoretical limit. The lack of progress in increasing Tc and Jc is due to a lack of understanding of the basic physics of these materials.

The current invention shows how significantly higher Tc and Je can be achieved in the cuprate materials class and in other materials with metallic and insulating regions. Such materials are of immense practical value in electrical machinery and power transmission.

SUMMARY OF THE INVENTION

To overcome the limitations described above, and to overcome other limitations that will become apparent upon reading and understanding this specification, one or more embodiments of the present invention disclose a superconducting composition of matter comprising a first region and a second region. The first and second regions comprise unit cells of a solid (e.g., crystalline or amorphous lattice, periodic or aperiodic lattice), the first region comprises an electrical insulator or semiconductor, the second region comprises a metallic electrical conductor. The second region extends or percolates through the solid (e.g., crystalline or amorphous) lattice and a subset of the second region comprises surface metal unit cells that are adjacent to at least one unit cell from the first region. The ratio of the number of the surface metal unit cells to the total number of unit cells in the second region being; at least 20 percent.

Examples of materials for the first region include an antiferromagnetic insulator, a non-magnetic insulator, and a semiconductor.

In one or more examples, the first region is comprised of metal-monoxides, MgO, CaO, SrO, BaO. MnO, FecO, CoO, NiO, CdO, EuO, PrO, or UO, and the second region is comprised of TiO, VO, NbO, NdO, or SmO.

In one or more further examples, the first region is comprised of Al₂O₃, and the second region is formed by replacing the Al atoms in the first region with Ti, V, or Cr atoms.

In yet further examples, the first region is comprised of V₂O₃ with up to 20% of the V atoms replaced by Cr atoms, and the second region is comprised of (V_(x)Ti₁-_(x))₂O₃ where x is greater than or equal to zero or less than or equal to one.

In yet further examples, in the composition of one or any combination of the previous examples, the second region is formed by replacing one type of atom in said first region by another type of atom of a different chemical valence.

In yet other examples, in the composition of one or any combination of the previous examples, the second region is formed by adding a type of atom to a subset of the unit cells of said first region, the type of atom of such chemical valence that the type of atom acts as an electrical donor or acceptor when added to said unit cells.

In further examples, in the composition of one or any combination of the previous examples, the second region is formed by adding interstitial atoms in said first region.

In yet other examples, in the composition of one or any combination of the previous examples, the first region is formed by replacing one type of atom in said second region by another type of atom of a different chemical valence.

In one or more examples, in the composition of one or any combination of the previous examples the first region is formed by adding a type of atom to a subset of the unit cells of said second region, the type of atom of such chemical valence that the type of atom acts as an electrical donor or acceptor when added to said unit cells.

In further examples, in the composition of one or any combination of the previous examples, said first region is formed by adding interstitial atoms in said second region.

In one or more examples, in the composition of one or any combination of the previous examples the second region is comprised of approximately linear subregions. For example, the approximately linear subregions of the second region can surround regions of the first kind (first region). In other examples, some of the surrounded regions of the first kind (first region) have atomic substitutions, grain boundaries, or interstitial atoms.

The present disclosure further describes a superconductor from the hole-doped cuprate class comprising two distinct atoms (first and second atoms) having such chemical valence that the first atom when added to the cuprate acts as an electrical acceptor, the second atom acts as an electrical donor, and 20% or at least 20% of said second atoms reside inside the unit cell between two of the first atoms that are a distance of two unit cells from each other. In one or more examples, the superconductor has the composition of one or any combination of the previous examples having the first and second regions (the second region including the distinct atoms).

The present disclosure further describes a superconducting composition of matter comprised of YB_(a2)Cu₃O_(6+x) where at least 5% of the Y atoms are replaced by +2 oxidation state atoms, Mg, Ca, Sr, Zn, Cd, Cu, Ni, or Co, at least 2% of the Y atoms are replaced by +4 oxidation state atoms, Ti, Zr, Hf, C, Si, Ge, Sn, or Pb. In one or more examples, the superconducting composition of matter has the composition of one or any combination of the previous examples having the first and second regions.

The present disclosure further describes a superconductor from the electron-doped cuprate class comprising two distinct atoms (first and second atoms) having such chemical valence that the first atom when added to the cuprate acts as an electrical donor, the second atom acts as an electrical acceptor, and 20% of said second atoms reside inside the unit cell between two of the first atoms that are a distance of two unit cells from each other. In one or more examples, the superconductor has the composition of one or any combination of the previous examples having the first and second regions (the second region including the distinct atoms).

The materials characteristics that are relevant for fabricating room-temperature superconductors and high current densities are also described.

BRIEF DESCRIPTION OF THE DRAWINGS

Referring now to the drawings in which like reference numbers represent corresponding parts throughout:

FIG. 1A and FIG. 1B illustrate the difference in the character of the doped hole using the “physicist's” density functionals, LDA and PBE (FIG. 1A), versus the “chemist's” hybrid density functionals (FIG. 1B). The dopant is negatively charged and resides out-of-the CuO₂ plane. The physicist's hole state has density in the CuO₂ plane and is delocalized over the crystal. It is a peculiar hole state. Intuitively, one would expect the positive hole charge to point at the negatively charged dopant. The chemist's hole state density is out-of-the-CuO₂ plane (points at dopant), and is localized around the four-Cu-site plaquette beneath the dopant. In the chemist's view, the crystal has atomic-scale inhomogeneity that is not a small perturbation of translational symmetry. The physicist's view leads to an approximately homogeneous crystal.

FIG. 2 . The doped four-Cu-site plaquette “motif”.

FIGS. 3A-3D illustrate the mechanism for the creation of delocalized planar metallic wavefunctions inside a doped plaquette. FIG. 3A shows the Cu d_(x2-y2) and O pσ orbital energies in an undoped plaquette. The energy ordering, ε_(x2-y2)<ε_(pσ)<ε_(x2-y2)+U, where U is the large on-site Cu d_(x2-y2) Coulomb repulsion leads to localization of the spins on the Cu sites, and hence the undoped AF state. FIG. 3B shows the Fermi Level for a doped plaquette. FIG. 3C shows the induced delocalization (shaded overlay) of the planar Cu d_(x2-y2) and O pσ electrons in the plaquette from the decrease of the Cu d_(x2-y2) orbital energy relative to the O pσ orbital energy. The decrease occurs because the positive charge of the chemist's out-of-the-plane hole from FIGS. 1B and 2 is closer to the planar Cu site than the planar O site. The out-of-plane hole is not shown here. There are a total of 4 O atom pσ orbitals and 4 Cu d_(x2-y2) orbitals inside the four-Cu-site plaquette. Since there are two spin states for each orbital, there is a total of (4+4)×2=16 states in the shaded overlay in the bottom right figure. These 16 states are filled with the 12 electrons (4 red plus 8 blue) shown in the lower left FIG. 3D.

FIG. 4 illustrates a 2D percolating pathway in an optimally doped CuO₂ plane (x=0.16 dopants per planar Cu). The black line shows a pathway from the left to the right side of this 40×40 CuO₂ lattice. The localized antiferromagnetic (AF) spins on the Cu sites are shown as black dots in the white region. The blue dots are Cu sites inside the doped metallic region. The O atoms are not shown. The yellow overlay represents the delocalized metallic band comprised of planar orbitals inside the doped region. The blue squares represent isolated plaquettes (not adjacent to another plaquette). There is a degeneracy at the Fermi level inside each isolated plaquette that is split by its interaction with the crystal environment, and thereby leads to the pseudogap [11]. The number of isolated plaquettes “vanish” (become of measure zero) at hole doping x≈0.19 where the cuprate pseudogap is known to disappear [11]. The tenuous percolating pathway has poor critical current.

FIGS. 5A-5C illustrate the character of the out-of-plane hole inside a doped plaquette. The arrows show, the displacement of the O atoms in the CuO₂ plane with each “frozen dumbbell” configuration. Proposed herein is that the out-of-plane hole wavefunction is a dynamic Jahn-Teller state that is a linear superposition (resonance) of the two dumbbells shown in FIGS. 5A and 5B (called a “fluctuating dumbbell”). The two frozen dumbbells in FIGS. 5A and 5B are represented schematically by the left and right figures in FIG. 5C. The fluctuating dumbbell is shown in the center figure in FIG. 5C. The shaded overlay represents the planar Cu d_(x2-y2) and O pσ electrons (not shown) that are delocalized inside the plaquette.

FIGS. 6A-6D illustrate the effect of overlapping piaquettes on the fluctuating dumbbells for the case of Sr doping of L_(a2-x)Sr_(x)CuO₄ FIG. 6A illustrates two non-overlapping plaquettes with fluctuating dumbbells, the CuO₂ layer and the out-of-the-plane Sr dopants. The schematic FIG. 6B shows the metallic delocalization of the planar Cu d_(x2-y2) and O pσ orbital electrons (shaded overlay) and the two fluctuating dumbbells. FIG. 6C shows two overlapping plaquettes. The degeneracy of the two dumbbell states inside each plaquette is broken and the two dynamic Jahn-Teller fluctuating dumbbells become two frozen dumbbells. FIG. 6D shows a schematic of the metallic regions (shaded overlay) and the frozen dumbbells. The orientation of the dumbbells in this figure is arbitrary. The actual orientation in the crystal will depend on the environment.

FIG. 7 . Plaquette doping at x=0.23 on a 40×40 CuO₂ lattice. The black dots are undoped AF Cu sites. The O atoms are not shown. The shaded (yellow) overlay represents the delocalized metal comprised of planar Cu d_(x2-y2) and planar O pσ character. Fluctuating dumbbells (crosses) are seen in non-overlapped plaquettes. The overlapped plaquettes are shown as squares (square outline, blue). There are frozen dumbbells inside each shaded square. The frozen dumbbells are not shown in the figure.

FIG. 8 . Plaquette doping of x=0.12 on a 40×40 CuO₂ lattice. The black dots are undoped AF Cu sites. No O atoms are shown. The squares are isolated plaquettes (no neighboring plaquette). The shaded (yellow) overlay represents the metallic region comprised of planar Cu d_(x2-y2) and planar O pσ character. Fluctuating dumbbells (crosses) are seen in non-overlapped plaquettes. The darker shaded (magenta) clusters are smaller than the Cooper pair coherence length and do not contribute to superconducting pairing. Since the size of a single plaquette (the Cu—Cu distance) is 3.8 Angstroms and the superconducting coherence length is ˜2 nm, we have chosen plaquette clusters fewer than or equal to 4 plaquettes in size to be fluctuating. The darker shaded (magenta) overlay means there is metallic delocalization of the planar Cu and O orbitals in these clusters. The isolated plaquettes do not contribute to the superconducting pairing and the superconducting fluctuations above Tc because they contribute to the pseudogap.

FIGS. 9A-9D. Plaquette doping of a 40×40 square CuO₂ lattice for dopings x=0.00 (FIG. 9A), 0.02 (FIG. 9B), 0.05 (FIG. 9C), and 0.10 (FIG. 9 )). Only the Cu sites are shown. The black dots are undoped AF Cu sites. The blue outlined squares are isolated plaquettes (no neighboring plaquette). The shaded (yellow) plaquette clusters are larger than 4 plaquettes in size (larger than the coherence length), and thereby contribute to the superconducting pairing. The darker shaded (magenta) clusters are metallic clusters that are smaller than the coherence length. The blue and green crosses are the fluctuating dumbbells. There is no plaquette overlap in this doping range.

FIGS. 10A-10D. Plaquette doping at x=012 (FIG. 10A), 0.15 (FIG. 10B), 0.16 (FIG. 10C), and 0.18 (FIG. 10D). The caption of FIGS. 9A-9D explains the symbols in this figure. Optimal Tc occurs for x≈0.16 (FIG. 10C) because the product of the size of the metallic region (number of electrons that can participate in superconducting pairing) and the size of the interface (the number of pairing phonon modes) is maximized. Percolation in 2D occurs at x≈0.15 (FIG. 10B). In the finite lattice shown here, there is no 2D percolating metallic pathway for x=0.15. A 2D percolating pathway appears at x=0.16, as shown in FIG. 4 . The number of isolated plaquettes rapidly decreases over this doping range. By x=0.18 doping, there is only one isolated plaquette in its 40×40 lattice. At optimal doping, the percolation pathway is very tenuous. The maximum critical current density, Jc, will be much less than the maximum due to Cooper pair depairing. Using current fabrication methods, cuprates have a low Je at the highest Tc. Crossing continuous metallic pathwxays one plaquette in width would have both large Tc and Jc.

FIGS. 11A-11D. Plaquette doping of a 40×40 square CuO₂ lattice for dopings x=0.19 (FIG. 11A), 0.24 (FIG. 11B), 0.27 (FIG. 11C), and 0.32 (FIG. 11D). See the caption of FIG. 9 for an explanation of the symbols in this figure. The first plaquette overlap can be seen at 0.19 doping (blue squares with dark outline). The degeneracy of the two dumbbells states inside each overlapping plaquette has been broken. A frozen dumbbell configuration exists inside each overlapped plaquette. It is not drawn. At 0.27 doping, only isolated spins remain (black dots). At 0.32 doping, there are no localized spins remaining. The crystal is purely metallic, Only one isolated plaquette (blue square with dark outline and darker shaded (magenta) interior) remains at x=0.19 doping. The number of isolated plaquettes never vanishes entirely. Instead, their number becomes of measure zero above x≈0.19 doping and leads to the vanishing of the pseudogap at x≈0,19. At x=0.32, the critical current density, Jc, will be close to the Cooper pairing depairing limit since the metallic pathways through the crystal are not tenuous. However, there is no interface pairing, leading to Tc=0.

FIG. 12A shows the planar O atom phonon mode at the metal-insulator interface. Its displacement is planar and normal to the Cu—O—Cu along the metal-insulator interface. Displacement by δ leads to changes to the neighboring interface Cu d_(x2-y2) orbital energy by δε (δε>0), There are three kinds of Cu atoms, edge, convex, and concave. Similarly, there is a change in the Cu to Cu hopping matrix element −δt(δt>0). We choose δt to equal the average of the δt at each Cu.

FIG. 12B shows the planar O atom phonon mode in the insulating region adjacent to the metal-insulator interface. The displacement is planar and normal to the metal-insulator interface. The δε and δt are defined in the same way as in FIG. 12A. There is a δε for the metallic Cu closest to the O atom and two −δt for hopping to neighboring metallic Cu sites. The metallic screening of the O atom charge is not strong because it resides in the insulating AF region. Hence, the two δt are large. As illustrated herein, the vibrational energy of these two phonon modes is set to 60 meV. [18] See Table III.

FIG. 13 . Anharmonicity of the O atom phonon mode in FIG. 12A due to the difference of the electron screening in the metallic and insulating regions. For FIG. 12B, the shaded (yellow) overlay is shifted to the left.

FIGS. 14A and 14B illustrate scattering between Cooper pairs. FIG. 14A is a schematic representation and FIG. 14B shows the scattering matrix element between two Cooper pairs (ψ⬆, ψ⬇) and (ψ⬆, ψ⬇) with the exchange of a phonon. The two electrons in each pair are time-reversed partners. The symbol x with a horizontal line above the x means the complex conjugate of x. For scatterings in the vicinity of the Fermi level, the matrix element is always negative, leading to a superconducting pair wavefunction that is a linear superposition of Cooper pairs with the same sign, Such a pair wavefunction is called isotropic S-wave. Unfortunately, it is known that the cuprate pair wavefunction changes sign and is of D-wave form (more specifically, of d_(x2-y2) form). See Tc Concept 6 for a resolution to the problem.

FIG. 15 . Evolution of the S-wave and D-wave superconducting pairing wavefunctions as a function of the Coulomb pseudopotential, μ*. Typically, μ* is small, leading to S-wave pairing as seen on the left-side of the figure. The fluctuating dumbbells raise μ* to μ*˜μ by disrupting the metallic electrons from screening the bare Coulomb repulsion, μ. As μ* increases, the S-wave Tc decreases while the D-wave Tc remains unchanged as shown in the red and green Tc expressions for S and D-wave, respectively. As μ* approaches the “bare” Coulomb repulsion, μ, the D-wave Tc becomes the favored pair symmetry for the superconductor. The right-side of the figure applies to cuprates.

FIG. 16 . Comparison of Experimental and Computed Tc-domes. Bi₂Sr₂CaCOu₂O_(8-δ)(light blue solid circles [36]), YBa₂Cu₃O_(7-δ)(green circles [37]), Y_(1-y)Ca_(y)Ba₂Cu₃O_(7-δ). (dark blue circles [38]), La_(2-X)Sr_(x)CuO₄ (magenta squares [39]), Bi₂Sr₂CuO_(6-δ)(green diamonds [40] and solid blue triangles, [17]), 6% Zn doped YBa₂(Cu_(0.94)Zn_(0.06))₃O_(7-δ)(open red triangles [38]), and Tl₂Ba₂CuO_(6-δ)(solid red circles [41,42]). The dashed red line is the proposed Tl₂Ba₂CuO_(6-δ) curve by Hussey et al. [41,42] The solid black, magenta, and red lines are computed according to the present invention (see computational methods section).

FIG. 17 . Comparison of the computed and experimental Tc as a function of CuO₂ layers per unit cell. The experimental data points (open symbols and dashed lines) are from Mukuda et al. [2] Two theoretical Tc curves obtained using the present invention are shown (solid symbols and solid lines). All parameters, including the hole dopings in each CuO₂ layer, are in the computational methods section. The generalization of the Eliashberg equations for one CuO₂ plane to multi-layers is also described in the computational methods section. If the hole doping in each layer is the same, then the computed Tc curve would monotonically increase with the number of layers, n, and saturate for large n. Since the hole doping for the inner layers is less than the hole doping on the outermost layers (see Table V in the computational methods section), there are fewer interface O atom phonons that contribute to the high Tc in the inner layers. The maximum Tc occurs at three layers.

FIG. 18A shows two non-overlapped plaquettes with their fluctuating dumbbells and their metallic region (shaded region, yellow) for the case of Sr dopants in La_(2-x)Sr_(x)CuO₄ The bottom schematic shows the fluctuating dumbbells as crosses and the metallic region in yellow.

FIG. 18B shows that adding Sr dopant between the two plaquettes freezes the two fluctuating dumbbells while maintaining exactly the same metallic footprint. The S-wave Tc increases due to the decrease of the Coulomb pseudopotential while the D-wave Tc remains unchanged. The blue squares in the bottom schematic represent the frozen dumbbells. The added Sr dopant is shown by the red square. However, any atom that breaks the degeneracy of the dumbbell states will work instead. The shaded (yellow) metallic overlay is unchanged from FIG. 18A. The orientation of the frozen dumbbells is arbitrary in the figure because it depends on the environment (not shown).

FIG. 18C shows two adjacent plaquettes that are shifted by one lattice spacing. No plaquette can be added to freeze the dumbbells while maintaining the same metallic footprint.

FIG. 19 . The S-wave and D-wave Tc's as a function of overlapped plaquette fraction, f. The insets show the evolution of the frozen dumbbells (blue and red squares) for optimal doping of x=0.16. The metallic footprint is unchanged. The D-wave Tc is constant (the Coulomb pseudopotential, μ*, has no effect). The maximum S-wave Tc is 387.2 K and the D-wave Tc is 98.0 K. We assume μ* varies linearly with

f,μ*(f,iω _(n))=μ*_(Fluc) F(iω _(n))(1−f)+μ*_(BCS)

where μ*Fluc=7 (the fluctuating dumbbell μ*) μ*BCS=0.1 (atypical BCS value), and the cutoff

F(iω _(n))=ω _(Fluc) ²/(ω _(n) ² +ω _(Fluc) ²)

uses ωFluc=60 meV. The Eliashberg imaginary frequency, iωn, is defined in Appendix G In order to achieve 100% frozen dumbbells, “domino” doping as shown in FIGS. 18 a and b was used. We set δε=δt=0 30, 0 0.0, 0.15 eV for Edge, Convex, and Concave orbital and hopping energies, respectively. See the definitions in FIG. 12 , We used a larger δε than FIG. 16 and the computational methods section because δε should be greater than δt due to its proximity to the planar o atom. Since the D-wave Tc is weakly dependent on δε, our choices in FIG. 16 were very conservative. The S-wave Tc values for 100% frozen dumbbells for the black, magenta, and red curves in FIG. 16 at optimal doping are 280,1 K, 164.4 K, and 99.0 K, respectively. The corresponding D-wave Tc values are 92.2 K, 38.5 K, and 27.7 K. Hence, the S-wave Tc is in the range of 280-390 K.

FIG. 20 . The iconic H₂ dissociation curve in chemistry (inset) and the iconic cuprate phase diagram (larger black figure). Both figures show the regimes of delocalized, intermediate, and localized electronic states. For H₂, electron delocalization occurs near the equilibrium bond distance of 0.74 Angstroms where the effective hopping, t, is larger than the effective Coulomb repulsion, U, of the electrons (see inset in upper right corner). Molecules do not exist at the intermediate (magenta) region since the potential is not a local minimum. Similarly, semiconductors can be classified into delocalized (covalent) and localized (ionic) with a sharp transition in-between based upon their Fermi level stabilization at a semiconductor-metal interface [43]. In cuprates, the intermediate regime is where the optimal superconducting Tc occurs. In analogy to molecules and semiconductors, the present disclosure believes that cuprates are unstable here, and thereby “phase separate” into delocalized metallic and insulating magnetic AF regions. Finally, we intentionally avoided using the terms “weak correlation” and “strong correlation” in the figure. The word correlation means different things to different scientists. For chemists, the delocalized region (t>>U) is “weak electron correlation,” and the localized region (t<<U) is “strong electron correlation.” For physicists, cuprates are considered a “strong correlation” problem.

FIGS. 21A-21F. “Crowded” crossed wires that have high Tc and Jc. The crossed metallic wires are one plaquette in width. The symbols in the metallic wires are defined in FIGS. 18 and 19 , with one change solely for clarity. Here, the added dopant (solid (red) square) that overlaps two plaquettes (larger blue squares with darker outline) does not have a red square boundary. The black circles are undoped AF Cu spins. FIGS. 21-21C show crossed wires with 4×4, 2×4, and 2×2 AF spins, respectively, inside each interior region formed by the perpendicular wires on 20×20 CuO₂ lattices. FIGS. 21D-21F show the corresponding lattices that are randomly doped to approximately the same fraction of metallic unit cells as the crossed wires in FIGS. 21A-21C (x=014, 0.17, and 0.19). The Tc for each wire configuration is approximately equal to the S-wave Tc for an optimally doped system since the ratio of the surface metal cells to the total metal cells is 68%, 75%, and 80% for FIGS. 21A, 21B, and 21C, respectively. The ratio is ≈91% at random optimal doping. The Tc's of FIGS. 21A, 21B, and 21C are approximately 12%, 8%, and 6% less than the S-wave Tc at optimal doping. The Jc for FIG. 21A is (1/2)Jc,max, where Jc,max is the theoretical maximum of ˜2×10⁷ A/cm² for YBa₂Cu₃O_(7-δ). In FIG. 21B, Jc=(1/3)Jc,max and (1/2)Jc,max for currents along the x and y-axes, respectively. For FIG. 21C, Jc=(1/3)Jc,max. Random optimal doping leads to Jc˜10⁻²Jc,max (see FIG. 4 ).

FIGS. 22A-22B. Atomic substitution inside non-overlapping plaquettes can freeze dumbbells by breaking the dumbbell degeneracy inside the plaquette. FIGS. 22A-22B show 20×20 CuO₂ lattices with 4×4 AF interiors and crossing metallic wires one plaquette in width. In FIG. 22A, the solid (green) dots/circles show random atomic substitutions or interstitial atoms inside the plaquettes. The atomic substitutions may occur at the Cu atom in the plaquette (shown here), the O atoms inside the CuO₂ plaquette, or the apical O atom sites. The O atoms are not shown in the figure. In FIG. 22B, solid (green) dots/circles representing atomic substitutions or interstitial atoms in the insulating AF region are also shown. So long as these solid (green) dots circles do not disrupt the insulating behavior of these regions, the superconductivity will not be disturbed FIG. 22B may be easier to engineer than FIG. 22A because the solid (green) dots/circles are dispersed more randomly.

FIG. 23 . Plot of Tc as a function of number of overlapped plaquettes.

FIG. 24 . Flowchart illustrating a method of fabricating superconducting materials.

FIG. 25 . The change in the Tc-dome as a function of the minimum plaquette cluster size for superconducting pairing. The black curve is identical to the black Tc curve in FIG. 16 . All parameters are described in the computational methods section.

FIG. 26 . A surface O atom phonon mode. The change in Cu orbital energy for the Cu atom, δε_(L) for the left Cu atom, and δε_(R), for the right Cu atom due to the displacement of the surface O atom on the metal-insulator interface. −δt is the change in the hopping energy. The position of the left Cu atom is at R and the right Cu atom is at R+a. δε_(L), δε_(R), and St are functions of R as seen in FIG. 12A. We choose the energy of all the surface phonon modes to be the same and equal to ω_(ph).

FIG. 27 . The Perpendicular O atom phonon mode. The O atom is in the insulating AF region. The chain Cu—O—Cu—O—Cu is on the metal-insulator surface. The change in Cu orbital energy for the central Cu atom located at position R is δε. −δt(−) is the change in the hopping between the Cu site at R-a and R. −δt(+) is the change in the hopping between the Cu site at R+a and R. δε, δt(−), and δt(+) are functions of position R as seen in FIG. 27 . We choose the energy of all the perpendicular surface phonon modes to be the same and equal to ω_(ph). In this figure, the displaced O atom is on the y-axis while the Cu—O—Cu—O—Cu chain is along the x-axis. We choose the convention of labeling the phonon mode by the axis of the AF O atom. Hence, this figure is a y-axis O phonon mode.

DETAILED DESCRIPTION OF THE INVENTION

In the following description of the preferred embodiment, reference is made to the accompanying drawings, which form a part hereof, and in which is shown by way of illustration a specific embodiment in which the invention may be practiced. It is to be understood that other embodiments may be utilized and structural changes may be made without departing from the scope of the present invention.

Technical Description

The present disclosure describes a new composition of matter useful as high temperature superconductors. The compositions are fabricated from a wide range of materials including, but not limited to, cuprate superconductors.

1. First Example: Cuprate Superconductors

The highest superconducting transition temperature, Tc, at ambient pressure is 138 K in the Mercury cuprate HgBa₂Ca₂Cu₃O_(8+δ)(Hg1223 was discovered in 1993) with three CuO₂ layers per unit cell [1,2]. The longest time period between record setting Tc discoveries is the 17 years between Pb (1913 with Tc=7.2 K) to Nb (1930 with Tc=9.2 K). With the enormous increase in focus on superconductivity after the discovery of cuprates 30 years ago, the current 24 years without a new record at ambient pressure indicates we may be reaching the maximum attainable Tc.

The present disclosure shows this conclusion to be wrong, demonstrating that Tc can be raised above room-temperature to ≈400K in cuprates by precise control of the spatial separation of dopants. Hence, there still remains substantial “latent” Tc in cuprates. However, the proposed doping strategy and superconducting mechanism is not restricted to cuprates and may be exploited in other materials.

The room-temperature Tc result described herein is based upon four observations:

-   -   (1) Cuprates are intrinsically inhomogeneous on the atomic-scale         and are comprised of insulating and metallic regions. The         metallic region is formed by doping the material.     -   (2) A diverse set of normal state properties are explained         solely from the topological properties of these two regions and         their doping evolution.     -   (3) Superconductivity results from phonons at or adjacent to the         interface between the metallic and insulating regions.         Transition temperatures Tc˜100 K are possible because the         electron-phonon coupling is of longer-range than metals (nearest         neighbor coupling).     -   (4) These interface phonons explain the observed superconducting         properties and lead to our prediction of room-temperature         superconductivity.

Research and funding invested into finding the mechanism for cuprate superconductivity and higher Tc materials has led to more than 200,000 refereed papers [3]. After this mind-boggling quantity of literature, it would be unlikely that any unturned stones remain that could lead to the room temperature superconductivity properties described herein.

However, as illustrated herein, the majority of the cuprate community settled upon the incorrect orbital nature of the doped hole. This mistake led to Hamriltonians (Hubbard models) that overlook significant features.

A major reason for the early adoption of these Hubbard models for cuprates was due to computational results using the ab initio local density approximation (LDA) in density functional theory (DFT). While LDA is now deprecated, being replaced by the Perdew-Burke-Ernzerhof functional 141 (PBE), both functionals lead to exactly the same doped hole wavefunction in cuprates. These “physicist” functionals find the doped hole to be a de-localized wavefunction comprised of orbitals residing in the CuO₂ planes common to all cuprates [5-7]. Unfortunately, LDA and PBE both contain unphysical Coulomb repulsion of an electron with itself [8]. The “chemist” hybrid density functionals, invented in 1993 (seven years after the discovery of cuprate superconductivity), corrected for this self-Coulomb error, and thereby found the doped hole residing in a localized wavefunction surrounding the dopant atom with orbital character pointing out of the CuO₂ planes [9,10].

A. Electronic Structure

FIG. 1A illustrates the nature of doped holes using the “physicist's” picture and FIG. 1B illustrates the nature of doped holes using the “chemist's” picture. As described herein, the “chemist's” ab initio doped hole picture leads to eight electronic structure concepts that explain a vast array of normal and superconducting state phenomenology using simple counting. These eight structural concepts are described below.

-   -   1. Structural Concept 1: Cuprates are inhomogeneous on an         atomic-scale. The inhomogeneity is not a small perturbation to         translational symmetry. It must be included at zeroth order.     -   2. Structural Concept 2: The cuprate motif is a four-Cu-site         plaquette formed by each dopant, as shown in FIG. 2 . The         out-of-the-CuO₂ plane negative dopant is surrounded by an         out-of-the-CuO₂ plane hole. The hole is comprised of apical         Oxygen pz and planar Cu d_(3z) ²_r² character. There is also         some planar O pσ character that is not drawn.     -   3. Structural Concept 3: A tiny piece of metal is formed within         each plaquette from electron delocalization in the planar Cu         d_(x) ²-y² and O pσ(px and py) orbitals, as shown in FIG. 3C.         Delocalization occurs because the positive charge of the         out-of-plane hole lowers the Cu d_(x) ²-y² orbital energy         relative to the O pσ orbital energy. In contrast, these         electrons are localized in a spin-1/2 antiferromagnetic (AF)         state in an undoped plaquette.     -   4. Structural Concept 4: A metal is formed when the doped         plaquettes percolate through the crystal. When a         three-dimensional (3D) pathway of adjacent doped plaquettes is         created through the crystal (percolation of the plaquettes), a         metallic band comprised of planar Cu d_(x) ²-y² and O pσ         orbitals is created inside the percolating region. These         delocalized metallic wavefunctions do not have momentum, k, as a         good quantum number. Two-dimensional (2D) percolation occurs at         a higher doping; (x≈0.15 holes per planar Cu) than the start of         3D percolation (at x≈0.05 holes per planar Cu), as shown in FIG.         4 . The undoped (non-metallic) region remains an insulating         spin-1/2 AF. Thus, cuprates have both insulating and metallic         regions on an atomic-scale.     -   5. Structural Concept 5: The out-of-the-CuO₂ plane hole shown in         FIG. 1 and FIG. 2 is a dynamic Jahn-Teller distortion that is a         linear superposition of two “frozen dumbbell” states, as shown         in FIGS. 5A-5C The dynamic Jahn-Teller hole state is called a         “fluctuating dumbbell.”     -   6. Structural Concept 6: A fluctuating dumbbell can be frozen by         overlapping its plaquette with another plaquette, as shown in         FIGS. 6A-6D.     -   7. Structural Concept 7: If possible, plaquettes avoid         overlapping. Since the dopant atom is negatively charged, two         plaquettes repel each other. Their Coulomb repulsion is         short-ranged because of screening from the planar metallic         electrons. Hence, plaquettes do not overlap, but are otherwise         distributed randomly. Plaquettes can avoid overlap up to a hole         doping of x=0.187. For dopings greater than x=0.187, plaquettes         must overlap, but as little as possible in order to minimize         their mutual repulsion. Up to x=0.187 doping, there always         exists a four-site square of AF spins where the next plaquette         can be placed. For the doping range 0.187<x<0.226, added         plaquettes can cover three AF spins. In the range 0.226<x<0.271,         plaquettes cover two AF spins, and from 0.271<x<0.316, a single         localized spin. At x=0.316, the crystal is fully metallic with         no localized spins. Further doping cannot increase the number of         metallic sites. FIG. 4 shows that plaquettes can avoid overlap         at x=0.16 doping. FIG. 7 shows x=0.23 doping, where plaquettes         must overlap.     -   8. Structural Concept 8: Plaquette clusters smaller than the         superconducting coherence length (2 nm) thermally fluctuate and         do not contribute to the superconducting pairing. At low         dopings, the plaquettes have not yet merged into a single         connected region. There exist plaquette clusters smaller than         the coherence length, as shown in magenta in FIG. 8 . They         cannot contribute to the superconducting Tc. These fluctuating         clusters lead to superconducting fluctuations above Tc.

FIGS. 9A-9D, 10A-10D, and 11A-11D show the evolution of the plaquettes as a function of doping. In the figures, the black dots 900 are undoped AF Cu sites, the blue outlined squares 902 are isolated plaquettes (no neighboring plaquette), the shaded (yellow) plaquette clusters 904 are larger than 4 plaquettes in size (larger than the superconducting coherence length), and thereby contribute to the superconducting pairing, and the darker shaded (magenta) clusters 906 are metallic clusters that are smaller than the coherence length. The blue and green crosses 908 are the fluctuating dumbbells. Squares 910 are overlapping plaquettes.

Only twelve dopings are shown here from the range x=0.00 to x=0.32. The Appendix in the provisional application 62/458,740 has similar figures for all dopings in this range in 0.01 increments (Figures S0-S32). Only one CuO₂ plane is shown in each of these figures.

B. Experimental Confirmation of the Electronic Structure Picture

The above identified eight electronic structural concepts explain a diverse set of normal state cuprate phenomenology as a function of doping by simple counting arguments [11-14]. These include the following results.

-   -   1. The low and high-temperature normal state resistivity by         counting the number of overlapped plaquettes and the size of the         metallic region [12,13]     -   2. For La_(2-x)Sr_(x)CuO₄ the fluctuating dumbbells in adjacent         CuO₂ layers become decorrelated above ˜1 K. Phonon modes with         character predominantly inside these plaquettes become 2D,         leading to the low-temperature linear resistivity term. For the         double-chain cuprate, YBa₂Cu₄O₈, if the fluctuating dumbbells         between adjacent CuO₂ layers are correlated, then these phonons         remain 3D, leading to a low-temperature resistivity that is         quadratic in temperature. as observed [15].     -   3. The pseudogap and its vanishing at x≈0.19 doping from         counting isolated plaquettes (not adjacent to another doped         plaquette in the same CuO₂ plane) and their spatial distribution         [11,12].     -   4. As discussed in Appendix B of the provisional application         62/458,740, there is a degeneracy near the Fermi level of the         planar states inside an isolated plaquette. The degeneracy is         broken by interaction with the environment. A nearby isolated         plaquette strongly splits the degeneracy and leads to the         pseudogap.     -   5. The “universal” room-temperature thermopower by counting the         sizes of the insulating AF and metallic regions and taking the         weighted average of the thermopower of each region [12,14].         Since the room-temperature thermopower of the AF region is ˜100         μV/K and the metallic region thermopower is ˜−10 μV/K, there is         a rapid decrease in the thermopower as the size of the metallic         region increases with doping.     -   6. The STM doping incommensurability by counting the size of the         metallic regions [12,14],     -   7. The energy of the (π, π) neutron spin scattering resonance         peak by counting the size of the AF regions [12,14]. The         resonance peak arises from the finite spin correlation length of         the AF regions.

Explanation of Superconducting Tc

The present disclosure uses exactly the same doped electronic structure described above to explain the superconducting Tc and its evolution with doping. The Oxygen atom phonon modes at and adjacent to the interface between the insulating and metallic regions lead to superconductivity. The magnitude of the electron-phonon coupling is estimated and the following results are obtained:

-   -   1. A large Tc˜100 K from phonons (because the range of the         electron-phonon coupling near the metal-insulator interface         increases from the poor metallic screening);     -   2. The observed Tc-dome as a function of hole doping (since the         total pairing is the product of the size of the metallic region         times the interface size);     -   3. The large Tc changes as a function of the number of CuO₂         layers per unit cell (from inter-layer phonon coupling of the         interface O atoms plus inhomogeneous hole doping of the layers);     -   4. The D-wave symmetry of the superconducting Cooper pair         wavefunction (also known as the D-wave superconducting gap). In         general, an isotropic S-wave superconducting pair wavefunction         is energetically favored over a D-wave pair wavefunction for         phonon-induced superconductivity. However, the fluctuating         dumbbells reduce the S-wave Tc below the D-wave Tc by         drastically increasing the Cooper pair electron repulsion.     -   5. The lack of a superconducting Tc isotope effect at optimal         doping (due to the random anharmonic potentials of each pairing         O atom);     -   6. By overlapping plaquettes, the fluctuating dumbbells become         frozen and the S-wave pair wavefunction Tc rises above the         D-wave Tc, as shown in FIG. 19 . FIG. 19 shows that, while         maintaining the same metallic “footprint” of optimal doping         (x=0.16), completely frozen dumbbells lead to an S-wave Tc of         ≈400 K when the D-wave Tc=100 K.

C. Superconducting Transition Temperatures

All the superconducting transition temperatures described herein are computed using the strong coupling Eliashberg equations [16] as detailed in Appendix G of the provisional application 62/458,740. These equations include the electron “lifetime” effects that substantially decrease Tc from the simple BCS Tc expression.

These results are shown in the following set of Tc Concepts.

-   -   1. Tc Concept F: FIGS. 12A-12B show there are two planar O atom         phonon modes (one at the metal- AF insulator interface and the         other adjacent to the interface on the insulating side) that         have longer-range electron coupling due to poor electron         screening from the metallic region. Hereinafter, the “effective”         single band model for the metallic band [17] is used. In this         model, the planar O atoms are eliminated. The model has a single         effective Cu d_(x) ²-y² orbital per Cu in the CuO₂ plane with an         effective hopping to neighboring metallic Cu atoms. The         parameters of the band structure are the Cu d_(x) ²-y² orbital         energy and the hopping terms (Table II, Appendix F in the         provisional application 62/458,740).     -   2. Tc Concept 2: The typical magnitude of the electron-phonon         coupling matrix element. g, is the geometric mean [16] of the         Debye energy, ωD, and the Fermi energy, E_(F), or g=√ωDE_(F).         The derivation is given in Appendix D in the provisional         application 62/458,740. For 0.02 eV<ωD<0.1 eV and E_(F)=1 eV,         0.14 eV<g<032 eV. All Tc results described herein use         electron-phonon coupling parameters in this range.     -   3. Tc Concept 3: FIG. 13 shows the potential energy of each O         atom in FIG. 12A is strongly anharmonic due to the difference of         the electron screening in the metallic and insulating regions.         In fact, the phonon mode shown in FIG. 12A is anharmonic even         without a nearby metal-insulator boundary. The “floppiness” of         the bond-bending of a linear chain (here, the planar Cu—O—Cu         chain) has been emphasized by Phillips [19] and seen by neutron         scattering (the F atom [20] in ScF₃ and the Ag atom [21] in         Ag₂O). However, without the metal-insulator boundary, reflection         symmetry would force the electron-phonon coupling for this mode         to be zero.     -   4. Tc Concept 4: Near optimal doping, x≈0.16, there is no Tc         isotope effect. Harmonic potentials have no isotope variation of         the superconducting pairing strength because the pairing is         inversely proportional to Mω² where M is the O atom mass and ω         is the angular frequency of the phonon mode. For a derivation of         this result, substitute

g=√{square root over ((h/Mω))}∇V

into the pairing coupling in FIG. 14B, where V is the electron potential.

Since

Mω²=K, where K is the spring constant, there is no pairing isotope effect. For anharmonic potentials, the phonon pairing strength becomes dependent on the isotope mass [22]. Anharmonic potentials can decrease or increase the Tc isotope effect depending on the details of the anharmonicity [23-25]. Near optimal doping, the metallic and insulating environments for each O atom phonon is random, leading to an average isotope effect of zero, as has been observed [26.27]. The O atom environment becomes less random at lower dopings, as seen in FIGS. 9A-9D. Hence, the isotope effect appears at low dopings [26,27].

-   -   5. Tc Concept 5: Cooper pairing from phonons is maximally phase         coherent for an isotropic S-wave pair wavefunction because the         sign of the pairing matrix element in FIG. 14B is always         negative. However, a D-wave pair wavefunction is observed for         cuprates. It appears prima facie that phonons cannot be         responsible for superconductivity in cuprates. Since Cooper         pairs are comprised of two electrons in time-reversed states,         the sign of the Cooper pair scattering is always negative and of         the form [28,29]

˜(−)|g| ² /hω _(ph)

where g is the matrix element to emit a phonon and hw_(ph) is the energy of the phonon mode (see FIG. 14A, 14B). Hence, the lowest energy superconducting pairing wavefunction is a linear superposition of Cooper pairs with the same sign, called the isotropic “S-wave” state. In theory, the pair Coulomb repulsion, μ, could suppress the S-wave state and lead to a D-wave state because μ cancels out of Tc when performing the angular integral around the D-wave pair wavefunction. However, the electrons in a pair can couple via a phonon while avoiding each other (due to retardation of phonons). The “effective” repulsion,μi*, known as the Morel-Anderson pseudopotential [16,28-32] is too small to raise the D-wave Tc higher than the S-wave Tc. Unless there is a mechanism for drastically increasing μ*, any phonon model for cuprate superconductivity is bound to fail to obtain the correct superconducting pair wavefunction. However, as shown here in Tc concept 6 below, the fluctuating dumbbells in FIG. 5 increase μ* to μ*˜μ, leading to a D-wave pairing wavefunction.

-   -   6. Tc Concept 6: FIG. 15 illustrates how the fluctuating         dumbbells suppress the S-wave pairing wavefunction and lead to a         D-wave pairing wavefunction. The expression for the         Morel-Anderson Coulomb pseudopotential [16,28-32]μ* (also shown         in FIG. 15 ) depends on the ratio of the Coulomb and phonon         energy scales as ω_(Cout)/ω_(phonon). Since this ratio is large,         μ* is small, leading to an S-wave pair wavefunction rather than         the experimentally observed D-wave pair wavefunction [33]. The         fluctuating dumbbell frequency, ω_(Dumbell), is of the same         order as ω_(phonon) because of the dynamic Jahn-Teller         distortion of the planar O atoms in FIG. 5 . The O atom         distortion disrupts the metallic screening of the Coulomb         repulsion, and thereby increases μ* as shown in FIG. 15 . In         essence, ω_(Dumbell) substitutes for ω_(cout) in the expression         for μ*. When μ*˜μ, a D-wave pair wavefunction is formed.     -   7. Tc Concept 7: Interface O atom-phonon pairing explains the         experimental Tc domes. FIG. 16 shows the calculated Tc-domes         versus experiment as a function of doping for different cuprates         using the phonon modes from FIG. 12 and the electron-phonon         couplings estimated in Tc Concept 2. All three computed D-wave         Tc domes were obtained from the strong-coupling Eliashberg         equations for Tc [16,34,35], Other phonon modes also contribute         to Tc. These phonons primarily reduce the magnitude of Tc due to         their contribution to electron pair “lifetime effects” (strictly         speaking, the “wavefunction renormalization effects”). The         effect of all the phonon modes on Tc is included in the         computations described herein. All the details of the band         structure, the interface O phonon coupling parameters, and the         inclusion of the remaining phonons into the Eliashberg         calculations are described in appendices F and G in the         provisional application 62/458,740. The parameters were         intentionally chosen to be simple and conceptual and we did not         attempt to fit the experimental points exactly. A goal of the         present disclosure is to demonstrate that reasonable         electron-phonon couplings and the proposed inhomogeneous cuprate         electronic structure are sufficient to understand the         experimental Tc-domes.     -   8. Tc Concept 8: The experimental variation of Tc with the         number of CuO₂ layers per unit cell is due to interlayer         coupling of the interface O atom-phonons and the nonuniform hole         doping between layers. Since the O atom phonons near the         metal-insulator interface are longer-ranged, they couple to         adjacent CuO₂ planes. Hence, there is a strong dependence of Tc         on the number of CuO₂ layers per unit cell. In addition, the Cu         Knight shift measurements of Mukuda et al [2] have shown that         the hole doping is not the same in each CuO₂ layer. The computed         Tc as a function of the number of CuO₂ layers is shown in FIG.         17 .     -   9. Tc Concept 9: The D-wave Tc values computed in FIGS. 16 and         17 are weakly dependent on the orbital energy change, δε, and         strongly dependent on the hopping energy change, δt. See Table I         for the change in Tc at optimal doping of x=0.16 for the         computed black, red, and magenta curves in FIG. 16 .

TABLE I The change in the Tc at optimal doping (x = 0.16) for the three computed curves in FIG. 16. The orbital energy parameter, δε, and the hopping energy parameter, δt, are each changed by 0% and ±10% from their initial values found in Appendix F. In appendices G2a and G2b, the δε terms lead to a more isotropic electron-phonon pairing, and the δt terms are more anisotropic. For a D-wave Tc, an isotropic electron- phonon pairing does not contribute to Tc. In the fourth column (red curve), δε = 0 (see Appendix F). Hence, changes to δε do not affect Tc. Black Magenta Change in Curve Curve Red Curve (δε, δt) YBa₂Cu₃O_(7-δ) La_(2-x)Sr_(x)CuO₄ YBa₂(Cu_(0.94)Zn_(0.06))₃O_(7-δ) (0%, 0%) 92.2 K 38.5 K 27.7 K (0%, −10%) 83.1 K 30.7 K 19.9 K (0%, +10%) 100.0 K  46.3 K 35.6 K (−10%, 0%) 93.6 K 39.4 K 27.7 K (−10%, 84.7 K 31.3 K 19.9 K −10%) (−10%, 101.1 K  47.5 K 35.6 K +10%) (+10%, 0%) 90.5 K 37.5 K 27.7 K (+10%, 81.4 K 30.1 K 19.9 K −10%) (+10%, 98.5 K 45.0 K 35.6 K +10%)

From Table 1, a 10% increase in δε always decreases the D-wave Tc, by ≈2-3%. A ±10% change in δt leads to ≈±10-30% change in the D-wave Tc. In appendices G2a and G2b, the exact dependence of the electron-phonon pairing parameter, λ, is derived. The contribution of δε to λ is approximately isotropic around the Fermi surface leading to a weak dependence of the D-wave Tc on changes in δε. In contrast, an S-wave pairing symmetry Tc depends strongly on both δε and δt. The weak dependence of the D-wave Tc on δε implies the δε parameters for the Tc curves in FIGS. 16 and 17 cannot be determined unambiguously from the experimental Tc data. The uncertainty in the magnitude of δε leads to an S-wave ‘T’c range from ≈270-400 K due to dopant “crowding,” as shown below.

-   -   10. Tc Concept 10: Overlapping plaquettes (“crowding” the         dopants) freeze the dumbbells, decrease the Coulomb         pseudopotential, μ*, and thereby raise the S-wave Tc. If the         same metallic “footprint” can be maintained, then there is no         change in the phonon pairing. Only μ* is reduced (see FIG. 15 ).         If all the dumbbells can be frozen, then from FIGS. 14 and 15 ,         the S-wave Tc will be larger than the D-wave Tc. FIGS. 18A-18C         shows how two plaquettes with fluctuating dumbbells can be         crowded by adding an additional dopant (Sr in the figure) while         retaining exactly the same metallic footprint. For random         doping, there will always exist adjacent plaquette pairs as         shown in FIG. 18C that cannot be overlapped by another plaquette         within the existing metallic footprint. There are two ways to         obtain an optimally doped metallic footprint and freeze 100% of         the dumbbells. First, dope “dominoes” (adjacent pairs of         plaquettes as in FIGS. 18A and 18B). Second. dope to less than         optimum doping. Next, crowd all of the plaquettes in such a way         as to end up with an optimally doped metallic footprint and 100%         frozen dumbbells.     -   11. Tc Concept 11: FIG. 19 shows crowding dopants while         maintaining the optimal doping metallic footprint leads to room         temperature S-wave Tc. In FIG. 20 , the ground state electronic         wavefunction of H₂ at the equilibrium bond separation of 0.74         Angstrom is well approximated by a restricted Hartree-Fock form         (a spin up and spin down electron pair occupying the same         bonding orbital). In the language of an effective electron         hopping, t, and an onsite Coulomb repulsion, U, this region is         represented by t>>U. At dissociation (t<<U), the ground state         electronic wavefunction is highly correlated. The wavefunction         is large only when there is one electron on each H atom. From         FIG. 20 , the optimal superconducting Tc of cuprates is at         “intermediate” correlation. Molecules do not generally “settle”         at intermediate correlation. Since the dopants in cuprates are         frozen in at high temperatures, the material avoids intermediate         correlation by phase separating on an atomic-scale into a         metallic (weak correlation) and insulating AF (strong         correlation) regions.

Atomic-scale inhomogeneity explains three important materials issues about cuprates. First, cuprates are known to “self-dope” to approximately optimal Tc. Since plaquette overlap occurs at x=0.187 doping, we believe it is energetically favorable for dopants to enter the crystal until their plaquettes begin to overlap. Adding further dopants is energetically unfavorable. The change in Tc between optimal doping (x≈0.16) and plaquette overlap (x=0.187) is ≈0.5%. Hence, cuprates “self-dope” to approximately optimal Tc as a consequence of the energetics of overlapping plaquettes.

Second, YBa₂Cu₃O_(7-δ) cannot be doped past x≈0.23, as shown in FIG. 16 . The phenomenon can be understood if it is energetically unfavorable to overlap plaquettes that share an edge (occurring at doping x=0,226). In the earliest days of cuprate supercon-ductivity, materials scientists had difficulty observing superconductivity in La_(2-x)Sr_(x)CuO₄ above ≈0.24 doping [44]. We believe the difficulty was also due to the energetics of overlapping plaquettes with shared edges. Annealing in an O₂ atmosphere solved the La_(2-x)Sr_(x)CuO₄ overdoping problem. However, the problem still remains for YBa₂Cu₃O_(7-δ).

Third, it is known that a room-temperature thermopower measurement is one of the fastest ways to determine if a cuprate sample is near optimal doping for Tc because the room-temperature thermopower is very close to zero near optimal doping. This peculiar, but useful, observation can be understood because 2D percolation of the metallic region occurs at x≈0.15 doping. Since the AF region thermopower is large (˜+100 μV/K) and the metallic thermopower is ˜−10 μV/K at high overdoping, 2D metallic percolation “shorts out” the AF thermopower and drives the thermopower close to zero near optimal Tc.

Finally, the potential energy curve in the intermediate correlation regime is hard to study for molecules. For H₂, the equilibrium bond distance is 0.74 Angstroms. The intermediate correlation regime is at ≈2.0 Angstrom bond separation. At this distance, the blue potential energy curve in FIG. 20 can only be observed indirectly [45-47] because it is not at a local minimum. For H₂, the ultraviolet spectrum of the vibrational modes (there are 14 discrete levels below the continuum) can be fitted to a simple Morse potential to estimate the potential energy as a function of the H—H separation distance. The 10th bond-stretching phonon mode probes the potential energy of the two of H atoms up to 2.0 Angstroms.

II. Second Example: General Materials Approaches to Room-Temperature Tc and Large Jc

As illustrated herein, there is enormous “latent” Tc residing in the cuprate class of superconductors from converting the D-wave superconducting pairing wavefunction to an S-wave pairing wavefunction. The result is surprising and unexpected because it has been assumed by most of the high-Tc cuprate community that there was something special about the D-wave pairing symmetry that led to Tc˜100 K.

Plaquettes have been overlapped with regularity for 30 years. However, these materials are all overdoped with doping x:>0.187, as shown in FIGS. 11A-11D. Hence, dumbbells have been frozen and the S-wave Tc has increased. However, the calculations presented herein find the S-wave Tc remains below the D-wave Tc for reasonable parameter choices. Unfortunately, the optimally doped metallic footprint is not obtained by naïve dopant crowding. Instead, the size of the metallic footprint increases and its pairing interface decreases. The right side of the Tc-dome shown in FIG. 16 is the result. Even the layer-by-layer Molecular Beam Epitaxy (MBE) of Bozovic et al. [48] does not control the placement of the dopants in each layer, leading to the same result as above.

While almost everything that can be possibly be suggested for the mechanism for cuprate superconductivity has been suggested in over 200,000 papers (percolation, inhomogeneity, dynamic Jahn-Teller distortions, competing orders. quantum critical points at optimal doping or elsewhere, spin fluctuations, resonating valence bonds, gauge theories, blocked single electron interlayer hopping, stripes, mid-infrared scenarios, polarons, bipolarons, spin polarons, spin bipolarons, preformed Bose-Einstein pairs, spin bags, one-band Hubbard models, three-band Hubbard models, t-J models, t+U models, phonons, magnons, plasmons, anyons, Hidden Fermi liquids, Marginal Fermi liquids, Nearly Antiferromagnetic Fermi liquids, Gossamer Superconductivity, the Quantum Protectorate, etc.), the inventor believes these ideas have lacked the microscopic detail necessary to guide experimental materials design, and in some instances, may have even led materials scientists down the wrong path.

As shown above (see FIG. 19 ), freezing dumbbells in cuprates leads to room-temperature Tc (see FIG. 19 ). However, the critical current density, Jc, is approximately two orders of magnitude smaller than the theoretical maximum, Jc˜10⁻²Jc,max, where Jc,max is the depairing limit for Cooper pairs. Jc is small because the conducting pathway in the CuO₂ planes is extremely tenuous (see the discussions in the captions of FIGS. 4 and 10 ). For practical engineering, Jc should be at least ˜10⁻¹ Jc,max.

In cuprates, Tc can be raised to room-temperature by freezing dumbbells while maintaining the random metallic footprint found at optimal doping. By fabricating wires (a wire is defined as a continuous 1D metallic pathway through the crystal), Tc remains large while Jc increases to at least ˜10⁻¹Jc,max.

The results presented herein lead to the following approaches for achieving higher Tc and Jc. Unless explicitly stated, the points below apply to any type of material (cuprate or non-cuprate).

1. The Material should be Inhomogeneous

The material should have a metallic region and an insulating region. The insulating region does not have to be magnetic. However, the inventor believes the antiferromagnetic insulating region helps maintain the sharp metal-insulator boundary seen in cuprates. An ordinary insulator or a semiconductor with a small number of mobile carriers is sufficient to obtain a longer ranged electron-phonon coupling at the interface because there is less electron screening in the semiconducting (or insulating) region compared to the metallic region. Thus, atomic-scale metal-insulator inhomogeneity in a 3D material leads to a high-Tc 3D S-wave pairing wavefunction. Moreover, a 3D material is more stable against defects and grain boundaries.

2. Ratio of Metallic Unit Cells

The ratio of the number of metallic unit cells on the interface (adjacent to at least one insulating unit cell) to the total number of metallic unit cells must be larger than 20%. The terms interface and surface are used interchangeably below. The number of metallic unit cells on the interface (or surface) must be a large fraction of the total number of metallic unit cells in order for the enhanced electron-phonon pairing at the interface to have an appreciable effect on Tc. From the calculations in FIG. 16 , 50% of optimal Tc is obtained when the ratio is ≈50%, and 25% of optimal Tc occurs when the ratio is =35%. Below a surface metal unit cells to total metal unit cells ratio of 20%, Tc falls off exponentially, and therefore Tc is too low to be useful.

3. Avoid Small Metallic Clusters

Metallic clusters that are smaller than approximately the coherence length do not contribute to Tc due to thermal fluctuations. The surface metal unit cells to total metal unit cells ratio described above should only include surface metal unit cells in extended metallic clusters.

In cuprates, high Tc can be obtained at very low doping if all the dopants leading to isolated plaquettes and small plaquette clusters are arranged such that a single contiguous metallic cluster is formed. While the Tc may be high, Jc will be low if the size of the metallic region is a small fraction of the total volume of the crystal.

Inhomogeneous materials formed at eutectic points have a surface metal unit cells to total metal unit cells ratio of ˜10⁻³ or less if the sizes of the metallic and insulating regions are on the order of microns. Standard materials fabrication methods do not lead to sufficient surface atomic sites for high Tc. Inhomogeneity on the atomic-scale is necessary.

4. Superconducting Wires Lead to a Small Increase of Tc and a Large Increase of Jc

It would appear that parallel 1D metallic wires that are one lattice constant wide (equal to one plaquette width in cuprates) would lead to the maximum surface unit cells to total metal unit cells ratio of 100%, and thereby a large Tc increase. It was surprising and unexpected to discover that at optimal doping of x=0.16, the surface metal unit cells to total metal unit cells ratio is 91% in cuprates, Increasing the ratio to 100% increases Tc by only ≈5% because at higher Tc magnitudes, Tc no longer increases exponentially with the magnitude of the electron-phonon coupling, λ. (defined in Appendix G). Instead, Tc scales [49] as Tc˜√λ. A 10% increase in the surface to total metal unit cells ratio increases λ by 10%, leading to a 5% in-crease in Tc. Hence, there is negligible Tc to be gained by fabricating wires.

While metallic wires lead to a tiny increase in Tc, metallic wires increase Je dramatically (up to a factor of ˜100) by eliminating the tortured conduction pathways shown in FIG. 4 . For cuprates, optimal Tc doping at x=0.16 is barely above the 2D percolation threshold of x≈0.15 doping. Hence, the conducting pathways in a single CuO₂ plane are tenuous at optimal doping.

Current materials fabrication methods for cuprates have optimized the Tc at the ex-pense of Jc. This point evidences that despite all the proposals in over 200,000 refereed publications [3] there has been little guidance to the materials synthesis community on what is relevant at the atomic level for optimizing Tc and Jc.

Parallel wires that are a few lattice constants in width are bad superconductors because 1D superconductor-normal state thermal fluctuations lead to large resistances below the nominal Tc. However, by fabricating two (or more) sets of parallel wires that cross each other, the effect of resistive thermal fluctuations in a single wire are suppressed. FIGS. 21-21F illustrate perpendicularly crossed wires in 21. In FIGS. 21A-21C, the added dopant (solid (red) square 2100) that overlaps two plaquettes (larger blue squares 2102 with darker outline) does not have a red square boundary (1802 and 1000 d) drawn for reasons of clarity only. The same pattern or a different pattern can be used in adjacent layers normal to the 2D wires. Crossing wires in 3D (two or more sets of parallel wires spanning the whole crystal) also leads to high Tc and Jc. Crossed metallic wires with varying aspect ratios and widths provide many opportunities for optimizing Tc and Jc for specific applications. For example, wires that are four metallic atoms wide (equal to two adjacent plaquettes in cuprates), would have ≈1/2 the surface to total metal ratio of metallic wires two atoms wide (or one plaquette in cuprates), leading to an 50% reduction in Tc compared to wires that are two metallic atoms wide. However, Jc increases by a factor of two.

Generally, it is most favorable to fabricate the narrowest wires that are spaced closely together because both Tc and Jc will be large. In addition, interfacial phonon modes will couple to both the closest wire and the next-nearest neighboring wire, leading to further increase in Tc. For cuprates, the narrowest wire is one plaquette width (see FIG. 2 ). Other materials will have a different minimum width scale for wires.

5. Dopants

In one or more examples, dopants are added to an insulating parent compound that leads to metallic regions. However, a metallic parent compound can also be doped to create insulating regions. In cuprates, the parent compound is insulating and doping creates metallic regions.

6. Metallic and Insulating Regions Provide New Opportunities for Pinning Magnetic Flux

Strong pinning of magnetic flux lines in superconductors is necessary to obtain large critical current densities, Jc. Insulating “pockets” surrounded by metallic region are energetically favorable for magnetic flux to penetrate. The flux can be strongly bound inside these insulating regions by adding further pinning centers to the insulating region. Examples of insulating pockets are shown in FIGS. 21A-21F.

7. Dumbell Freezing in Cuprates

In cuprates, it is desirable to freeze the fluctuating dumbbells in non-overlapping plaquettes while maintaining a metallic footprint with a large surface metallic unit cells to total metallic unit cells ratio. The ratio of the isotropic S-wave pairing wavefunction Tc to the corresponding D-wave Tc is ≈2.8-4 (see FIG. 19 ). In cuprates, fluctuating dumbbells in non-overlapping plaquettes can be frozen by breaking the symmetry inside each plaquette by an atomic substitution into the CuO₂ plane, atomic substitution out of the CuO₂ plane (such as the apical O atom sites), or interstitial atoms, as shown in FIGS. 22A-22B.

III. Experimental Methods

There are three materials issues with crowding dopants:

-   -   1. Tc does not increase with crowding until the D-wave gap         symmetry changes to S-wave at ˜20% crowding. Thus, Tc is not         useful as a metric for sample characterization.     -   2. Dopants are charged, and hence repel each other.     -   3. The optimal Tc metallic footprint at 0.16 holes per CuO₂         plane (the shaded (yellow) overlay 2300 in FIG. 23 ) must be         retained.

There are two cuprates materials where the dopant crowding idea can be tested:

La_(2-x)Sr_(x)CuQ₄:

As illustrated herein, the Tc of optimally doped La_(2-x)Sr_(x)CuQ₄ increases from 40 K with no dopant crowding (f=0.0 in FIG. 23 ) to Tc˜160 K with 100% crowding (f=1.0). This material does not lead to room-temperature Tc. However, the crowding method described below is simple.

The ionic charges of the La and Sr atoms in La_(2-x)Sr_(x)CuO₄ are +3 and +2 (or −1 relative to La⁺³), respectively. The most direct way to crowd dopants is to add atoms with a. +1 charge relative to La⁺³ (a +4 oxidation state) because they favor residing in-between the Sr⁺² atoms due to charge attraction. At first glance, it appears this approach is counter-productive because a +4 atom adds an electron, and thereby lowers the net doping and T_(c). However, the added electron fills a hole in the out-of-plane fluctuating dumbbells rather than doping the planar CuO₂ metallic band. The net result is our desired crowding. Example crowding dopants include C⁺⁴, Sr⁺⁴, Ge⁺⁴, Sn⁺⁴, Ti⁺⁴, Zr⁺⁴, Hf⁺⁴, and Pt⁺⁴. These dopants are smaller than La⁺³, and hence will “fit” in-between the two Sr atoms.

YBa₂Cu₃O_(6+x):

FIG. 23 shows Tc for YBCO as a function of crowding. Tc reaches ˜390K. Since Oxygen is added to the chains instead of atomic substitution as in LSCO, the LSCO crowding method above does not apply to YBCO. In one fabrication method. O atoms may be removed from the chains (lowering x) and substituting Ca atoms for Y in order to bring the material back to optimal doping. This substitution has already been shown to work experimentally. Hence, Ca becomes the equivalent of Sr in LSCO. At this point, the crowding method for LSCO can be used for (YCa)CuO.

The lack of any change in Tc for dopant crowding less than 20% and the counter-intuitive suggestion above of electron doping the material are the reasons the materials community did not “accidentally” find this room-temperature mechanism, despite intense effort over 31 years.

In one or more examples, the room-temperature Seebeck coefficient (thermopower) of new material samples can be tested because it is a direct measure of the size of the metallic regions (yellow overlay in FIG. 23 ), and it can be done cheaply in a few minutes. The goal is to add +4 dopants beyond optimal doping without changing the Seebeck coefficient. This approach will lead the materials scientists up the red dotted curve in FIG. 23 , and thereby into the solid red region where Tc is large.

TV. Process Steps

FIG. 24 is a flowchart illustrating a method of fabricating a superconducting composition/state of matter 1000 (referring also to FIGS. 10C, 18B, and 19 ).

Block 2400 represents combining a first region 1002 a or material and a second region 1002 b or material to form a composition of matter 1000.

In one or more examples, the first region 1002 a or material and the second region 1002 b or material each comprise unit cells 1004 a, 1004 b, respectively, of a solid 1000 c (e.g., crystalline or amorphous lattice). The second region 1002 b extends through the solid (e.g., crystalline or amorphous lattice) and a subset of the second region 1002 b are surface metal unit cells 1004 b that are adjacent to at least one unit cell 1004 a from the first region 1002 a. The ratio of the number of the surface metal unit cells 1004 b to the total number of unit cells 1004 b, 906, 902 in the second region 1002 b is at least 20 percent (e.g., in a range of 20%-100%).

The first region 1002 a or material comprises an electrical insulator or semiconductor. Examples of insulator include an antiferromagnetic insulator or a non-magnetic insulator. The second region or material comprises a metallic electrical conductor.

Examples of the composition of matter 1000 include the first region or material 1002 a comprising at least one compound selected from the metal-monoxides, MgO, CaO, SrO, BaO, MnO, FeO, CoO, NiO, CdO, EuO, PrO, and UO, combined with the second region or material 1002 b comprising at least one compound selected from TiO, VO, NbO, NdO, and SmO.

Further examples of the composition of matter 1000 include the first region 1002 a or material comprising at least one compound selected from V₂O₃ with up to 20% of the V atoms replaced by Cr atoms, combined with the second region 1002 b comprised of (V_(x)Ti_(1-x))₂O₃ where x is greater than or equal to zero or less than or equal to one.

Yet further examples of the composition 1000 include the first region 1002 a comprised of Al₂O₃ and the second region 1002 b is formed by replacing the Al atoms in the first region with Ti, V, or Cr atoms.

In yet further examples, the second region 1002 b is formed by replacing one type of atom in the first region 1002 a by another type of atom of a different chemical valence.

In yet further examples, the second region 1002 b is formed by adding a t_(y)pe of atom to a subset of the unit cells 1004 a of the first region 1002 a, the type of atom of such chemical valence that (when the type of atom is added to the unit cells 1004 a) the type of atom acts as an electrical donor or acceptor.

In one or more examples, the second region 1002 b is formed by adding interstitial atoms in said first region 1002 a.

In yet further examples, the first region 1002 a is formed by replacing one type of atom in the second region 1002 b by another type of atom of a different chemical valence.

In yet further examples, the first region 1002 a is formed by adding a type of atom to a subset of the unit cells 1004 b of the second region 1002 b, the type of atom of such chemical valence that (when the type of atoms is added to the unit cells) the type of atom acts as an electrical donor or acceptor.

In yet further examples, the first region 1002 a is formed by adding interstitial atoms in the second region 1002 b.

In yet further examples, the combining comprises combining two distinct atoms (first 1800 and second atoms 1802). The first atom 1800 (e.g., Sr) has a chemical valence such that when the first atom 1800 is added to the material (e.g., cuprate), the first atom 1800 acts as an electrical acceptor. The second atom 1802 (e.g., Ti) has a chemical valence such that, when the second atom is added to the material (e.g., cuprate), the second atom 1802 acts as an electrical donor, and 20% or at least 20% (e.g., 20%-100%) of said second atoms 1802 reside inside the unit cell 1804 between two of said first atoms 1800 that are a distance of two unit cells 1804, 1000 d from each other. In on one or more examples, the second region 1002 includes the two distinct atoms (first 1800 and second atoms 1802) and the superconductor is from the hole-doped cuprate class.

In yet further examples, the combining comprises forming YBa₂Cu₃O_(6+x) where at least 5% of the Y atoms are replaced by +2 oxidation state atoms, Mg, Ca, Sr, Zn, Cd, Cu, Ni, or Co, at least 2% of the Y atoms are replaced by +4 oxidation state atoms, Ti, Zr, Hf, C, Si, Ge, Sn, or Pb.

In yet further examples, the combining comprises combining two distinct atoms (first and second atoms) having such chemical valence that (when added to the cuprate) the first atom acts as an electrical donor, the second atom acts as an electrical acceptor, and 20% or at least 20% (e.g., 20%-100%) of said second atoms reside inside the unit cell between two of the first atoms that are a distance of two unit cells from each other. In on one or more examples, the second region includes the two distinct atoms (first and second atoms) and the superconductor is from the electron-doped cuprate class.

In yet further examples, the second region 1002 a is comprised of approximately linear subregions 1010, as illustrated in FIG. 18B. The approximately linear subregions 1010 of the second region 1002 b can surround regions of a first kind or first region 1002 a. Some of the surrounded regions of the first kind/region 1002 a may have atomic substitutions, grain boundaries, or interstitial atoms.

In one or more examples, the components are provided in powder form and ground together in a pestle and mortar.

Block 2402 represents the step of doping the composition formed in Block 2400. Examples of doping include first n-type doping the composition then p-type doping the composition. Exemplary ranges of n-type doping include a doping concentration in a range from 5% up to 80% (e.g., 5% up to 20%) n-type dopants per unit cell Exemplary ranges of p-type doping include a doping concentration in a range from 5% up to 80% (e.g., 5% up to 20%) p-type dopants per unit cell. In one or more examples where the composition comprises a cuprate, the n-type doping and p-type doping are such that the dopant concentration x is in a range of 0.13-0.19. Examples of dopants include, but are not limited to, Mg, Ca, Sr, Zn, Cd, Cu. Ni, Co. Ti, Zr, Hf, C, Si, Ge, Sn, Pb.

In one or more examples, the dopants are provided in powder form and mixed together (e.g., ground together in a pestle and mortar) with the components of Block 2400.

Block 2404 represents the optional step of annealing the doped composite formed in Block 2402.

Block 2406 represents the optional step of measuring the insulator/semiconductor and metal content in the composition. In one or more examples, the step comprises measuring a thermopower of the composite, wherein the thermopower quantifies the amount of metal and insulator/semiconductor in the composition. The measurement enables identification of the fraction of overlapped plaquettes as a function of the structure, doping, and composition of the first region and the second regions, so that compositions mapping onto the red curve 2302 in FIG. 23 can be fabricated. Desired compositions are those measured with a ratio of the number of the surface metal unit cells to the total number of unit cells in the second region is at least 20 percent (e.g., in a range of 20-100%).

Block 2408 represents repeating steps 2400-2404 with modified compositions if the measurement in Block 2406 indicates that the fraction of overlapped plaquettes, f, does not lie on the S-wave curve in FIG. 23 so as to obtain the desired Tc.

Block 2410 illustrates the end result, a superconducting composition of matter having a Tc in a range of 100-400 K, wherein a ratio of the number of the surface metal unit cells to the total number of unit cells in the second region is at least 20 percent (e.g., in a range of 20-100%). In one or more examples, both the metallic content of the superconductor and the surface area of the metallic regions overlapping with the insulator/semiconductor regions are maximized.

Superconducting compositions of matter according to embodiments of the present invention may also be designed by computationally solving equations G43-G45 in the computational methods section for any combination of material(s) using the appropriate parameters for those materials.

V. Computational Methods and Approximations a. Estimate of the Magnitude of the Electron Phonon Coupling

It is known to be qualitatively correct that ℏw_(D)/E_(F)≈√{square root over (m/M)} where ℏw_(D) is the Debye energy, E_(F) is the Fermi energy, m is the electron mass, and M is the nuclear mass. One can quickly see that the form of the above expression is correct using ω_(D)˜√{square root over (K/M)} where K is the spring constant and K˜E_(F)k_(F) ²˜mE_(F) ²/ℏ² due to metallic electron screening.

The electron-phonon coupling, g, is of the form g˜√{square root over (ℏ/2Mω_(D))}∇V, where V is the nuclear potential energy. Substituting ∇V˜k_(F)E_(F), leads to g²˜(ℏ/2Mω_(D))k_(F) ²E_(F) ²˜(m/M)E_(F) ³/(ℏw_(D))˜(ℏw_(D))E_(F). Hence, g≈√{square root over (ℏω_(D)E_(F))}.

Another derivation is dimensional. The coupling, g, has dimensions of energy and there are only two relevant energy scales, ℏw_(D) and E_(F). Thus there are three possibilities for g. the mean, the geometric mean, and the harmonic mean of ℏω and E_(F). Since ℏω_(D)<<E_(F), the mean is ≈E_(F), and the harmonic mean is ≈ℏω_(D). Neither of these two means makes intuitive sense because we know metallic electrons strongly screen the nuclear-nuclear potential. The only sensible choice is the geometric mean, g˜√{square root over (ℏω_(D)E_(F))}.

b. Fluctuation Tc: Plaquette Clusters Smaller than the Coherence Length

There are superconducting fluctuations above Tc at low dopings due to the fluctuating magenta plaquette clusters in FIGS. 8, 9A-9D, and 10A-10D. These plaquette clusters have superconducting pairing that does not contribute to the observed Tc because the clusters are smaller than the coherence length. Including these clusters into the Tc computation leads to an estimate of the temperature range where plaquette cluster superconducting fluctuations occur above Tc. The resulting “fluctuation Tc domes” are plotted in FIG. 26 . Of course, there exist superconducting fluctuations above Tc from the plaquette clusters that are larger than the coherence length (yellow clusters 904 in FIGS. 8, 9A-9D, and 10A-10D). The fluctuation Tc from the larger yellow clusters is not included in FIG. 26 .

Parameters Used in the T_(c) Computations

TABLE II The planar Cu d_(x) ² ⁻

² and O p_(σ) band structure used in all T_(c) computations. We use effective single band parameters derived from the angle-resolved photoemission (ARPES) Fermi surface for single layer Bi2201.¹⁷ The 2D tight-binding band structure is ϵ_(k) = −2t[cos(k_(x)α) + cos(k

α)] − 4t′ cos(k_(x)α) cos(k

α) − 2t″[cos(2k_(x)α) + cos(2k

α)], where α is the planar Cu—Cu lattice size and the 2D momentum is k = (k_(x), k

). The ratio t″/t′ = −1/2 is assumed.¹⁷ The variable n in the table is the number of metallic electrons per metallic Cu. At optimal doping, the number of holes per metallic Cu in the CuO₂ plane is x = 0.16, leading to n = 1.0 − x = 0.84. The optimal doping Fermi level is used for all dopings in order to keep the number of parameters to a minimum. For the multi-layer T_(c) calculations in FIG. 17, we assume the 2D band structure ϵ_(k) above. The 2D k states in adjacent layers, l and l ± 1, are coupled by a momentum dependent matrix element equal to < k, l ± 1|H_(inter)|k, l >= −αt_(z)(1/4)(cos(k_(x)α) − cos(k

α))², where α is the product of the fraction of metallic sites in layers l and l ± 1. Since interlayer hopping of an electron between Cu sites on different layers can only occur if the two Cu sites are metallic, α is the probability of two adjacent Cu sites in different layers being metallic. The dopings of the individual layers in the multi-layer T_(c) calculations are all less than the threshold for plaquette overlap at x = 0.187. Hence, each plaquette covers 4 Cu sites. For example, between layers doped at x = 0.16 and x = 0.11, α = 4(0.16) × 4(0.11) = 0.2816 leading to αt_(z) ≈ 0.023 eV. n t (eV) t′ (eV) t_(z) (eV) 0.84 0.25 −0.05625 0.08

TABLE III Parameters that remain the same for every T_(c) calculation. They are the mass-enhancement parameter derived from the high-temperature linear slope of the resistivity, λ_(tr), the Debye energy, ℏw_(D), the minimum energy used in the low-temperature linear resistivity, ℏw_(min), the energy cutoff for Eliashberg sums, ℏw_(c), and the energy of the O atom phonon modes, ℏw_(ph). λ_(tr) (dimensionless) ℏw_(D) (Kelvin) ℏw_(min) (Kelvin) ℏw_(c) (eV) ℏw_(ph) (eV) 0.5 300 1.0 0.3 0.06

TABLE IV Parameters for the T_(c) curves in FIGS. 16, 17, and 26. The variable, N_(min), is the number of metallic Cu sites inside the smallest plaquette cluster that is larger than the coherence length, and thereby contributes to T_(c). The edge, convex, and concave couplings are chosen to be equal for the next layer couplings. All units are eV. δϵ δt Next Layer Figure Curve Color N_(min) Edge Convex Concave Edge Convex Concave δϵ_(NL) δt_(NL) 16 Black 20 0.150 0.150 0.075 0.240 0.240 0.120 16 Magenta 20 0.150 0.150 0.075 0.130 0.130 0.065 16 Red 100 0.000 0.000 0.000 0.132 0.132 0.000 26 Blue 8 0.150 0.150 0.075 0.240 0.240 0.120 26 Green 12 0.150 0.150 0.075 0.240 0.240 0.120 26 Red 16 0.150 0.150 0.075 0.240 0.240 0.120 26 Black 20 0.150 0.150 0.075 0.240 0.240 0.120 17 Black 20 0.150 0.150 0.075 0.240 0.240 0.120 0.0 0.2 17 Blue 20 0.050 0.000 0.000 0.130 0.130 0.065 0.05 0.13

TABLE V Doping of each CuO₂ layer in the multi-layer T_(c) calculations. The outermost layers are always at optimal doping (x = 0.16). The adjacent layers are at x = 0.11 doping. The innermost layers are all at x = 0.09 doping. These dopings are obtained from Cu Knight shift measurements.² Layers Hole Doping per CuO₂ Layer 1 0.16 2 0.16 0.16 3 0.16 0.11 0.16 4 0.16 0.11 0.11 0.16 5 0.16 0.11 0.09 0.11 0.16 6 0.16 0.11 0.09 0.09 0.11 0.16 7 0.16 0.11 0.09 0.09 0.09 0.11 0.16 8 0.16 0.11 0.09 0.09 0.09 0.09 0.11 0.16 9 0.16 0.11 0.09 0.09 0.09 0.09 0.09 0.11 0.16 10 0.16 0.11 0.09 0.09 0.09 0.09 0.09 0.09 0.11 0.16

Description of the Eliashberg T_(c) Calculations 1. The Eliashberg Equations

The attractive electron-electron pairing mediated by phonons is not instantaneous in time due to the non-zero frequency of the phonon modes (phonon retardation). In addition, electrons are scattered by phonons leading to electron wavefunction renormalization (“lifetime effects”) that decrease T_(c). Any credible T_(c) prediction must incorporate both of these effects. All T_(c) calculations in this paper solve the Eliashberg equations for the superconducting pairing wavefunction (also called the gap function). It includes both the pairing retardation and the electron lifetime.^(16,20,59)

The Eliashberg equations are non-linear equations for the superconducting gap function, Δ(k, ω, T), and the wave function renormalization, Z(k, ω, T), as a function of momentum k, frequency ω, and temperature T. Usually, the T dependence of Δ and Z is assumed, and they are written as Δ(k, ω) and Z(k, ω), respectively. We follow this convention here. Both Δ(k, ω) and Z(k,ω) are complex numbers. In this Appendix only, we will absorb Boltzmann's constant, k_(B) into T. Thus T has units of energy.

Both Δ and Z are frequency dependent because of the non-instantaneous nature of the superconducting electron-electron pairing. If the pairing via phonons was instantaneous in time, then there would be no frequency dependence to Δ and Z. The simpler BCS²⁹, gap equation assumes an instantaneous pairing interaction (Δ is independent of ω) and no wavefunction renormalization (Z=1).

The Eliashberg equations may be solved in momentum and frequency space (k, ω), or in momentum and discrete imaginary frequency space, (k, iω_(n)) where n is an integer and ω_(n)=(2n+1)πT. In the imaginary frequency space representation, the temperature dependence and the retardation of the phonon induced pairing are both absorbed into the imaginary frequency dependence, iω_(n). In theory, both Δ(k, ω) and Z(k, ω) can be obtained by analytic continuation of their (k iω_(n)) counterparts. In practice, the analytic continuation is fraught with numerical difficulties.⁶⁰⁻⁶³ However, the symmetry of the gap can be extracted from either the real or imaginary frequency representations of Δ.

In the pioneering work of Schrieffer, Scalapino, and Wilkins,^(29,34,35,59) the goal was to obtain the isotropic (in k-space) gap function at zero temperature, Δ(ω), as a function of ω in order to compute the superconducting tunneling of lead (T_(c)=7.2 K). Hence, they solved the full non-linear Eliashberg equations in frequency space.

Above T_(c), Δ(k,ω) is zero. For T≈T_(C), Δ is small. Since our interest in this paper is on the magnitude of T_(c) and the symmetry of the superconducting gap, we can linearize the gap, Δ, in the Eliashberg: equation for temperatures, T, close to T_(c), The result is a temperature dependent real symmetric matrix eigenvalue equation with Δ(k, ω) as the eigenvector. The eigenvalues are dimensionless and the largest eigenvalue mnonotonically increases as T decreases. For T>T_(c), the largest eigenvalue of the real symmetric matrix is less than 1. At T=T_(c), the largest eigenvalue equals 1, signifying the onset of supe rconductivity.

The non-linear Eliashberg equations (or the linearized version) are easier to solve in imaginary frequency space.^(≠)Hence, we solve the linearized Eliashberg equations in imaginary frequency space to obtain T_(c).

We use the linearized Eliashberg equations as derived in the excellent chapter by Allen and Mitrovic.¹⁶ Prior Eliashberg formulations assume translational symmetry (momentum k is a good quantum number for the metallic states). Our metallic wavefunctions are not k states because they are only non-zero in the percolating metallic region. We write the wavefunction and energy for the state with index l as Ψ_(i) and ∈_(i), respectively. Since Ψ_(i) is only delocalized over the metallic region and is normalized, Ψ_(i)˜1/√{square root over (N_(M))}, where N_(M) is the total number of metallic Cu sites. Rather than Cooper pairing occurring between k⬆ and its time-reversed partner, −k⬇, a Cooper pair here is comprised of (Ψ_(i)⬆, Ψ_(i) ⬇), where Ψ_(i) is the complex conjugate of Ψ_(i).

The linearized Eliashberg equations for Δ(I, iω_(n)) and Z(I, iω_(n)) are obtained from the k-vector equations-¹⁶ simply by replacing k writh the index I everywhere

$\begin{matrix} {{{Z\left( {l,{i\omega_{n}}} \right)} = {1 + {\frac{\pi T}{❘\omega_{n}❘}{\sum\limits_{l^{\prime}n^{\prime}}^{{❘\omega_{n}^{\prime}❘} < \omega_{c}}{\left\lbrack \frac{\delta\left( {\epsilon_{l}^{\prime} - \epsilon_{F}} \right)}{N(0)} \right\rbrack{\lambda\left( {l,l^{\prime},{\omega_{n} - \omega_{n}^{\prime}}} \right)}s_{n}s_{n}^{\prime}}}}}},} & ({G1}) \end{matrix}$ $\begin{matrix} {{{{Z\left( {l,{i\omega_{n}}} \right)}{\Delta\left( {l,{i\omega_{n}}} \right)}} = {\pi T \times {\sum\limits_{l^{\prime}n^{\prime}}^{{❘\omega_{n}^{\prime}❘} < \omega_{c}}{{{\frac{1}{❘\omega_{n}^{\prime}❘}\left\lbrack \frac{\delta\left( {\epsilon_{l}^{\prime} - \epsilon_{F}} \right)}{N(0)} \right\rbrack}\left\lbrack {{\lambda\left( {l,l^{\prime},{\omega_{n} - \omega_{n}^{\prime}}} \right)} - {u^{*}\left( \omega_{c} \right)}} \right\rbrack}{\Delta\left( {l^{\prime},{i\omega_{n}^{\prime}}} \right)}}}}},} & ({G2}) \end{matrix}$

where ∈_(F) is the Fermi energy, N(0) is the total metallic density of states per spin per energy, s_(n)=ω_(n)/|ω_(n)|=sgn(ω_(n)) is the sign of ω_(n), ω_(c) is the cutoff energy for the frequency sums, λ(I, I′, ω_(n)) is the dimensionless phonon pairing strength (defined below), and μ*(ω_(c)) is the dimensionless Morel-Anderson Coulomb pseudopotential at cutoff energy ω_(c). It is a real number. The wavefunction renormalization, Z(l, iω_(n)), is dimensionless. In the non-linear Eliashberg equations, Δ(I,iω_(n)) is has units of energy. In the linearized equations above, Δ(l,iω_(n)) is an eigenvector and is arbitrary up to a constant factor.

The “electron-phonon spectral function” α²F(l, l′, Ω) is defined

$\begin{matrix} {{{\alpha^{2}{F\left( {l,l^{\prime},\Omega} \right)}} = {{N(0)}{\sum\limits_{\sigma}{{❘{< l}❘}H_{ep}^{\sigma}{❘{l^{\prime} >}❘}^{2}{\delta\left( {\omega_{\sigma} - \Omega} \right)}}}}},} & ({G3}) \end{matrix}$

and the phonon pairing strength λ(l, l′, ω_(n)) is defined

$\begin{matrix} {\lambda\left( {l,l^{\prime},\omega_{n}} \right)} & = & {\int_{0}^{+ \infty}{d\Omega\alpha^{2}{F\left( {l,l^{\prime},\Omega} \right)}\left( \frac{2\Omega}{\omega_{n}^{2} + \Omega^{2}} \right)\,}} & ({G4}) \\  & = & {{N(0){\sum\limits_{\sigma}{{❘{< l}❘}H_{ep}^{\sigma}{❘{l^{\prime} >}❘}^{2}\left( \frac{2\omega_{\sigma}}{\omega_{n}^{2} + \omega_{\sigma}^{2}} \right)}}},} & ({G5}) \end{matrix}$

where <l|H_(ep) ^(σ)|l′>is the matrix element (units of energy) between initial and final states l′ and l, respectively of the electron-phonon coupling, and H_(ep) ^(σ) is the electron-phonon coupling for the phonon mode σ with energy ω_(σ). Both α²F(l, l′, Ω) and λ(l, l′, ω_(n)), are real positive numbers. Hence, Z(l, iω_(n)) is a real positive number. From G2, the gap Δ(l, iω_(n)) can always be chosen to be real. Since λ(l, l′, ω_(n))=λ(l, l′, −ω_(n)) from equation G4.

Z(l,−iω _(n))=Z(l,iω _(n))=Real Number,  (G6)

Δ(l,−iω _(n))=Δ(l,iω _(n))=Real Number.  (G7)

α²F(l, l′, Ω) and λ(l, l′, ω_(n)) are dimensionless because (eV)⁻¹ (eV)²(eV)⁻¹˜1. Physically, they should be independent of the number of metallic Cu sites N_(M), as N_(M) becomes infinite. The independence with respect to N_(M) is shown below.

The electron-phonon Hamiltonian for phonon mode σ, H_(ep) ^(σ), is

$\begin{matrix} {{H_{ep}^{\sigma} = {\left( \frac{\hslash}{2M\omega_{\sigma}} \right)^{\frac{1}{2}}{\nabla{V\left( {a_{\sigma} + a_{\sigma}^{\dagger}} \right)}}}},} & ({G8}) \end{matrix}$

where M is the nuclear mass, a_(σ) and a_(σ) ^(†) destroy and create σ phonon modes, respectively. V is the potential energy of the electron. For localized phonon modes, ∇V is independent of the number of metallic sites, N_(M). The l and l′ metallic states each scale as 1/√{square root over (N_(M))}, leading to <l|H_(ep) ^(σ)|I′>˜1/N_(M). Since the number of localized phonon modes scales as N_(M), the N_(M), scaling of the sum Σ_(σ)|<I|H_(ep) ^(σ)|I′>|² is ˜N_(M)(1/N_(M))²˜1/N_(M). Hence, we have shown that α²F(l, l′, Ω) and λ(I, I′,ω_(n)) are dimensionless and independent of N_(M) because the density of states per spin, N(0), is proportional to N_(M). In fact, α² F and λ are independent of N_(M) even when the phonon modes σ are delocalized. In this case, ∇V˜1/√{square root over (N_(M))}. The electron-phonon matrix element <l|H_(ep) ^(σ)|l′>is now summed over the crystal, and thereby picks up a factor of N_(M). Hence, <l|H_(ep) ^(σ)|l′>˜N_(M)×√{square root over (1/N_(M))}×√{square root over (1/N_(M))}×˜√{square root over (1/N_(M))} For delocalized phonons, the sum over phonon modes σ in Σ_(σ)|<I|H_(ep) ^(σ)|l′>|² does not add another factor of N_(M). The claim is obvious when I and l′ are momentum states k and k′ because the only phonon mode that connects these two states has momentum q=k−k′. Therefore, α²F(l, l′, Ω) and λ(l, l′, ω_(n)) are always dimensionless and independent of N_(M).

The atomic-scale inhomogeneity of cnprates implies translation is not a perfect symmetry of the crystal. However, the dopants are distributed randomly, and therefore on average k becomes a good quantum number. Hence, we may work with Green's functions in k space and approximate the Cooper pairing to occur between (k ⬆, −k⬇) states. The approximation is identical to the very successful Virtual Crystal Approximation (VCA) and the Coherent Potential Approximation (CPA) for random alloys.⁶⁴

In the VCA and CPA, the Green's function between two distinct k states, k and k′ is zero

G(k,k′,iω _(n))≈0,if k≠k′.  (G9)

The fact that k is not a good quantum number of the crystal is incorporated by including a self-energy correction, Σ(k, iω_(n)) at zeroth order into the metallic Green's function

$\begin{matrix} {{G\left( {k,{i\omega_{n}}} \right)} = {\frac{1}{{i\omega_{n}} - {\epsilon_{bare}(k)} - {\sum\left( {k,{i\omega_{n}}} \right)}}.}} & ({G10}) \end{matrix}$

Here, ∈_(here)(k) is the bare electron energy. Σ(k, iω_(n)) can be written as the sun of two terms, Σ(k, iω_(n))=Σ₀(k, iω_(n))+iω_(n)Σ₁(k, iω_(n)). Both Σ₀ and Σ₁ are even powers of ω_(n) Σ_(i)(k, −iω_(n))=Σ_(i)(k, iω_(n)), for i=1, 2. Σ₀ adds a shift to the bare electron energy, ∈_(here)(k), and a lifetime broadening to the electronic state. Σ₁ leads to wavefunction renormalization of the bare electron state.

The shift of ∈_(bare)(k) due to K₀(k, iω_(n)) leads to the observed angle-resolved photoemission (ARPES) band structure in cuprates,¹⁷ ∈_(k), and its lifetime broadening. The lifetime broadening integrates out of the Eliashberg equations because the integral of a Lorentzian across the Fermi energy is independent of the width of the Lorentzian.¹⁶ Hence, we may use the ARPES band structure, ∈_(k), in the Eliashberg equations and absorb Σ₁(k, iω_(n)) into Z(k, iω_(n)) in the Eliashberg equations.

Hence, we are right back to the standard Eliashberg equations^(16,29,34,35,59)

$\begin{matrix} {{{Z\left( {k,{i\omega_{n}}} \right)} = {1 + {\frac{\pi T}{❘\omega_{n}❘}{\sum\limits_{k^{\prime}n^{\prime}}^{{❘\omega_{n}^{\prime}❘} < \omega_{c}}{\left\lbrack \frac{\delta\left( {\epsilon_{k}^{\prime} - \epsilon_{F}} \right)}{N(0)} \right\rbrack{\lambda\left( {k,k^{\prime},{\omega_{n} - \omega_{n}^{\prime}}} \right)}s_{n}s_{n}^{\prime}}}}}},} & ({G11}) \end{matrix}$ ${{{Z\left( {k,{i\omega_{n}}} \right)}{\Delta\left( {k,{i\omega_{n}}} \right)}} = {\pi T \times {\sum\limits_{k^{\prime}n^{\prime}}^{{❘\omega_{n}^{\prime}❘} < \omega_{c}}{{{\frac{1}{❘\omega_{n}^{\prime}❘}\left\lbrack \frac{\delta\left( {\epsilon_{k}^{\prime} - \epsilon_{F}} \right)}{N(0)} \right\rbrack}\left\lbrack {{\lambda\left( {k,k^{\prime},{\omega_{n} - \omega_{n}^{\prime}}} \right)} - {u^{*}\left( \omega_{c} \right)}} \right\rbrack}{\Delta\left( {k^{\prime},{i\omega_{n}^{\prime}}} \right)}}}}},$ $\begin{matrix} {{{Z\left( {k,{{- i}\omega_{n}}} \right)} = {{Z\left( {k,{i\omega_{n}}} \right)} = {{Real}{Number}}}},} & ({G12}) \end{matrix}$ $\begin{matrix} {{\Delta\left( {k,{{- i}\omega_{n}}} \right)} = {{\Delta\left( {k,{i\omega_{n}}} \right)} = {{Real}{{Number}.}}}} & ({G13}) \end{matrix}$

The Eliashberg equations above are completely general for a single band crossing the Fermi level. The only inputs into the equations are the Fermi surface, Fermi velocity (in order to obtain the local density of states), the dimensionless electron-phonon pairing, (k, k′, ω_(n)), and the dimensionless Morel-Anderson Coulomb pseudopotential at the cutoff energy (typically, chosen to be five times larger than the highest phonon mode, ω_(c)=5ω_(ph)), μ*(ω_(c)). We apply the standard methods¹⁶ to map the above equations into a matrix equation for the highest eigenvalue as a function of T. The highest eigenvalue monotonically increases at T decreases. When the highest eigenvalue crosses 1, T_(c) is found.

Equations G11, G12, G13 need to be modified when more than one band crosses the Fermi level. Phonons can scatter electron pairs from one band to another in addition to scattering within a single band. The modification to the single Fermi surface Eliashberg equations above require changing the k and k′ labels to bk and b′k′ where b and b′ refer to the band index. k and k′ remain vectors in 2D so long as we assume the coupling of CuO₂ layers in different unit cells is weak. The number of bands is equal to the number of CuO₂ layers per unit cell, L. We derive the electron-phonon pairing λ for a single layer cuprate in sections G2 and G3. In section G4, we derive the multi-layer λ.

The total electron-phonon spectral function is the sum of four terms

α ² F=+60 ² F ₁ +α ² F ₂ +α ² F _(surf) +α ² F _(⊥),  (G221)

where α²F₁ and α²F₂ are the spectral functions from phonons that contribute to the resistivity. α²F₁ is due to the phonons that lead to the low-temperature linear term in the resistivity, and α²F₂ is due to the phonons that lead to the the low-temperature T² resistivity term.⁶⁵ α²F_(surf) is the component due to the planar O atom at the surface between the metal and insulating regions. It is the O atom phonon shown in FIG. 12 a α²F_(⊥) is the contribution from the planar O atom adjacent to the metal-insulator surface on the insulating AF side. It is shown in FIG. 12 b . Since the energy of these two O phonons modes is ≈60 meV,¹⁸ their contribution to the resistivity is very small.

Sections G2 and G3 in this Appendix derive the four α²F terms above in order to obtain the total phonon pairing, λ=λ₁+λ₂+λ_(surf)+λ_(⊥), that is used in the Eliashberg equations G11, G12, and G13 for T_(c).

2. Contribution to λ from the Interface O Atom Phonons

The Hamiltonian for FIG. 26 is

H _(surf) (R)=δ∈_(L) C _(L) ^(†) C _(L)+ϵ_(R) C ^(†) _(R)−δt(C ⁵⁵⁴ _(L) C _(R)+C ^(†) _(R) C _(L))  (G15)

where c^(†) _(L) and C_(L) create and destroy an electron at the L Cu site. c^(†) _(R) and C_(R) are defined similarly. Since there is no electron spin coupling to the) atom phonon mode the electron spin index is dropped in equation G15.

The k state ϕ(k) is defined as

$\begin{matrix} {{{\phi(k)} = {N_{M}^{- \frac{1}{2}}{\sum\limits_{R}{e^{{ik} \cdot R}{\phi(R)}}}}},} & ({G16}) \end{matrix}$

where ϕ(R) is the localized effective Cu d_(x) ²-y² orbital at position R, and N_(M) the number of metallic Cu sites. The matrix element between k′ and k is

$\begin{matrix} {\left\langle {\phi\left( {k^{\prime}{❘{H_{surf}(R)}❘}{\phi(k)}} \right.} \right\rangle = {N_{M}^{- 1}{e^{{- {i({k^{\prime} - k})}}{({R + {\frac{1}{2}a}})}}\left\lbrack {{\delta\epsilon_{L}e^{\frac{i}{2}{({k^{\prime} - k})}a}} + {\delta\epsilon_{L}e^{{- \frac{i}{2}}{({k^{\prime} - k})}a}} - {2\delta t\cos\frac{1}{2}\left( {k^{\prime} - k} \right)a}} \right\rbrack}}} & ({G17}) \end{matrix}$

The modulus squared is

$\begin{matrix} {{❘\left\langle {{\phi\left( k^{\prime} \right)}{❘{H_{surf}(R)}❘}{\phi(k)}} \right\rangle ❘}^{2} = {N_{M}^{- 2}\left\{ {\left\lbrack {{\left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)\cos\frac{1}{2}\left( {k^{\prime} - k} \right)a} - {2\delta t\cos\frac{1}{2}\left( {k^{\prime} + k} \right)a}} \right\rbrack^{2} + {\left( {{\delta\epsilon}_{L} - {\delta\epsilon}_{R}} \right)^{2}\sin^{2}\frac{1}{2}\left( {k^{\prime} - k} \right)a}} \right\}}} & \left( {G18} \right) \end{matrix}$

Define the two functions of k and k′. J_(surf) ^((x))(k, k′) and J_(surf) ^((y))(k, k′) as

$\begin{matrix} {{{J_{surf}^{(x)}\left( {k,k^{\prime}} \right)} = {{\left\langle \left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)^{2} \right\rangle_{x}\cos^{2}\frac{1}{2}\left( {k_{x}^{\prime} - k_{x}} \right)a} - {2\left\langle {\delta{t\left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)}} \right\rangle_{x}\cos\frac{1}{2}\left( {k_{x}^{\prime} - k_{x}} \right)a\cos\frac{1}{2}\left( {k_{x}^{\prime} + k_{x}} \right)a} + {{\left\langle {\delta t^{2}} \right\rangle_{x} \cdot 4}\cos^{2}\frac{1}{2}\left( {k_{x}^{\prime} + k_{x}} \right)a} + {\left\langle \left( {{\delta\epsilon}_{L} - {\delta\epsilon}_{R}} \right)^{2} \right\rangle_{x}\sin^{2}\frac{1}{2}\left( {k_{x}^{\prime} - k_{x}} \right)a}}},} & \left( {G19} \right) \end{matrix}$ $\begin{matrix} {{{J_{surf}^{(y)}\left( {k,k^{\prime}} \right)} = {{\left\langle \left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)^{2} \right\rangle_{y}\cos^{2}\frac{1}{2}\left( {k_{y}^{\prime} - k_{y}} \right)a} - {2\left\langle {\delta{t\left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)}} \right\rangle_{y}\cos\frac{1}{2}\left( {k_{y}^{\prime} - k_{y}} \right)a\cos\frac{1}{2}\left( {k_{y}^{\prime} + k_{y}} \right)a} + {{\left\langle {\delta t^{2}} \right\rangle_{y} \cdot 4}\cos^{2}\frac{1}{2}\left( {k_{y}^{\prime} + k_{y}} \right)a} + {\left\langle \left( {{\delta\epsilon}_{L} - {\delta\epsilon}_{R}} \right)^{2} \right\rangle_{y}\sin^{2}\frac{1}{2}\left( {k_{y}^{\prime} - k_{y}} \right)a}}},} & \left( {G20} \right) \end{matrix}$

where F(R_(σ))>_(x), is the average of the function F(R_(σ)) defined for each planar surface O on the x-axis with Position R_(σ) as shown in FIG. 26 ,

$\begin{matrix} {\left\langle {F\left( R_{\sigma} \right)} \right\rangle = {\frac{1}{N_{M}}{\sum\limits_{R_{\sigma}}{{F\left( R_{\sigma} \right)}.}}}} & \left( {G21} \right) \end{matrix}$

similarly, <F(R_(σ))>,

is the average of F(R_(σ)), over the y-axis surface O atoms. The

expression in equation G20 for

is identical to the expression for J_(surf) ^((π)) in equation G19 with x replaced by

From the k-space versions or equations G3 and G4

$\begin{matrix} {{\lambda_{surf}\left( {k,k^{\prime},\omega_{n}} \right)} = {{\left( \frac{N(0)}{N_{M}} \right)\left\lbrack {{J_{surf}^{(x)}\left( {k,k^{\prime}} \right)} + {J_{surf}^{(y)}\left( {k,k^{\prime}} \right)}} \right\rbrack}{\left( \frac{2\omega_{ph}}{\omega_{n}^{2} + \omega_{ph}^{2}} \right).}}} & \left( {G22} \right) \end{matrix}$

b. O Atom Mode Perpendicular to Surface

The Hamiltonian for FIG. 27 is

H⊥(R)=δ∈C ^(†) _(R) C _(R) −δt(−)(c ^(†) _(R−a) C _(R) +C ^(†) _(R) C _(R−a))−δt(+)(C ^(†) _(R+a) C _(R) +C ^(†) _(R) C _(R+a));  (G23)

where c_(R) ^(†) and c_(R) create and destroy an electron at the R Cu site. c^(†) _(R+a) and c_(R+a) are defined similarly. Since there is no electron spin coupling to the O atom phonon node, the electron spin index is dropped in equation G23.

The matrix element between k′ and k is

(ϕ(k′)|H⊥(R)|ϕ(k))=N _(M) ⁻¹ e ^(−i(k′−k)R) [δ∈−δt(+)(e ^(−ik′a) +e ^(ika))−δt(−)(e ^(ik′a) +e ^(−ika))]  (G24)

The modulus squared is

|(ϕ(k′)H⊥(R)|ϕ(k))|² =N _(M) ⁻² {{δ∈−[δt(+)+δt(−)][cos(k′a)+cos(ka)]}²

+[δt(+)−δt(−)]²[sin(k′a)−sin(ka)]²}  (G25)

Define the two functions of k and k′, J_(⊥) ^((x)) (k, k′) and J_(⊥) ^((y)) (k k′) as

J _(⊥) ^((x))(k,k′)=

δ∈²

_(x)−2

δ∈[δt(+)+δt(−)]

_(x)(cos k′ _(x) a+cos k _(x) a)

+

[δt(+)+δt(−)]

_(x)(cos k′ _(x) a+cos k _(x) a)²

+

[δt(+)−δt(−)]

_(x)(sin k′ _(x) a−sin k _(x) a)²,  (G26)

J _(⊥) ^((y))(k,k′)=

δ∈²

_(y)−2

δ∈[δt(+)+δt(−)]

_(y)(cos

a+cos k

a)

+

[δt(+)+δt(−)]

_(y)(cos

a+cos k _(y) a)²

+

[δt(+)−δt(−)]

_(y)(sin k′ _(y) a−sin k _(y) a)²,  (G27)

where <F(R_(σ))>_(x) is the average, defined in equation G21, of the function F(R_(σ)) for each x-axis Qphonon node with position R_(σ) a shown in FIG. 27 . Similary, <F(R_(σ))

is the average of F(R_(σ)) over the y-axis Oatoms. lie expression in equation G27 for J^((y)) is identical to the expression for J_(⊥) ^((x)) in equation G26 with x replaced by y.

From the k-space versions of equations G3 and G4

$\begin{matrix} {{\lambda_{\bot}\left( {k,k^{\prime},\omega_{n}} \right)} = {{\left( \frac{N(0)}{N_{M}} \right)\left\lbrack {{J_{\bot}^{(x)}\left( {k,k^{\prime}} \right)} + {J_{\bot}^{(y)}\left( {k,k^{\prime}} \right)}} \right\rbrack}{\left( \frac{2\omega_{ph}}{\omega_{n}^{2} + \omega_{ph}^{2}} \right).}}} & \left( {G28} \right) \end{matrix}$

3. Contribution to λ from the Phonons Responsible for the the Resistivity

The low-temperature resistivity of La_(2-x)Sr_(x)CuO₄ is the sum of two terms.⁶⁵ One term is linear in T and the other is proportional to T2. At high temperatures, both terms become linear in T. Previously, we showed¹³ that the doping evolution of these two terms can be explained by phonon scattering and simple counting of the number of metallic sites and the number of overlapped plaquettes, as a function of doping. The contribution of these phonons on T_(c) must be included in our Eliashberg calculation.

The power law dependence of the two terms in the resistivity restricts the form of their electron-phonon spectral functions, α²F₁ and α²F₂ for the linear and T² contributions, respectively. From Fermni's Golden Rule, the electron scattering rate is

$\begin{matrix} {{\frac{1}{\tau(k)} = {\frac{2\pi}{\hslash}{\sum\limits_{k}{2{\int}_{0}^{+ \infty}d{\Omega\alpha}^{2}{F\left( {k,k^{\prime},\Omega} \right)}{n_{B}(\Omega)}}}}},} & \left( {G29} \right) \end{matrix}$

where n_(B) (Ω) is the Bose-Einstein distribution n_(B)(ω)=: 1/[exp(ω/T)−1]. The factor of two in front of the integral cones from the absorption and emission of phonons. α²F is zero for Ω greater than the highest phonon energy.

At high temperatures, n_(B)(Ω)≈T/Ω leading to h/T(k)≈2πλ_(k)T, where

$\begin{matrix} {{\lambda_{k} = {2{\int}_{0}^{+ \infty}d\Omega\frac{\alpha^{2}{F\left( {k,\Omega} \right)}}{\Omega}}},} & \left( {G30} \right) \end{matrix}$

and α²F(k, Ω)=Σ_(k), α²F(k, k′, Ω). λ_(k) is called the mass-enhancement factor.¹⁶ The slope of the high-temperature scattering rate can be obtained from the resistivity. Hence, the mass-enhancement can be computed from experiment.

At low-temperatures, the Bose-Einstein distribution cuts the integral in the scattering rate off at Ω˜T. If α²F˜Ω^(n), then

$\begin{matrix} {\left. \frac{1}{\tau(k)} \right.\sim\left. {\int}_{0}^{T}d\Omega\frac{\alpha^{2}{F\left( {k,\Omega} \right)}}{\Omega}(T) \right.\sim{T^{n + 1}.}} & \left( {G31} \right) \end{matrix}$

The low-temperature T² scattering rate is known to be isotropic in k-space,⁶⁶ and thereby it must scale as ˜Ω from equation G31. From the low-temperature resistivity experiments⁶⁵. we showed. the T² resistivity term was proportional to (1−N_(4M)/N_(Tot)), where N_(Tot) is the total number of Cu sites (metallic plus insulating AF sites) and N_(4M) is the number of metallic Cu sites that are in non-overlapping plaquettes. Therefore, α²F₂(k, k′, Ω) is of the form

$\begin{matrix} {{{\alpha^{2}{F_{2}\left( {k,k^{\prime},\Omega} \right)}} = {{C_{2}\left( \frac{\Omega}{\omega_{D}} \right)}\left( {1 - \frac{N_{4M}}{N_{Tot}}} \right)}},} & \left( {G32} \right) \end{matrix}$

where C₂ is a constant to be determined. ω_(D) is the Debye energy. α²F₂=0, for Ω>ω_(D).

The low-temperature T scattering rate is zero along the diagonals, k_(T)=±ky, and large at k=(0, ±π). (±π, 0).⁶⁶ a²F₁ is independent of Ω from equation G31. The scattering rate in equation G31 logaritimically diverges for small Ω. Hence, it must be cutoff at some minimum, ω_(min). For temperatures below ω_(min), the scattering rate cannot be linear in T. Previously, we showed that ω_(min)≈1 K.¹³ In this paper, we fix ω_(min)=1 K. See Appendix F.

The spectral function, α²F₁(k, k′, Ω) is of the form

$\begin{matrix} {{{\alpha^{2}{F_{1}\left( {k,k^{\prime},\Omega} \right)}} = {{C_{1}\left( \frac{N_{4M}}{N_{Tot}} \right)}{D(k)}{D\left( k^{\prime} \right)}}},{{{for}\omega_{\min}} < \Omega < \omega_{D}},} & \left( {G33} \right) \end{matrix}$

where C₁ is a constant and α²F₁=0 outside of the range ω_(min)<Ω<ω_(D).

The anisotropy factor, D(k), is

$\begin{matrix} {{D(k)} = \frac{\left( {{\cos\left( {k_{x}a} \right)} - {\cos\left( {k_{y}a} \right)}} \right)^{2}}{\left\langle \left( {{\cos\left( {k_{x}a} \right)} - {\cos\left( {k_{y}a} \right)}} \right)^{2} \right\rangle}} & \left( {G34} \right) \end{matrix}$

where the denominator is the average over the Fermi surface of the numerator.

The average of a function, f(k), over the Fermi surface is defined as

$\begin{matrix} {\left\langle {f(k)} \right\rangle = {\frac{{{\sum}_{k^{\prime}}\left\lbrack \frac{\delta\left( {\varepsilon_{k^{\prime}} - \varepsilon_{F}} \right)}{N(0)} \right\rbrack}{f\left( k^{\prime} \right)}}{{\sum}_{k^{\prime}}\left\lbrack \frac{\delta\left( {\epsilon_{k^{\prime}} - \epsilon_{F}} \right)}{N(0)} \right\rbrack}.}} & \left( {G35} \right) \end{matrix}$

Thus <D(k)>=1.

The constants C₁ and C₂ can be determined as follows. The average around the Fermi surface of the scattering rate at high-temperatures is 1/T=2πλ_(tr)T. From resistivity measurements,⁶⁷λ_(tr)≈0.5. A fraction (N_(4M)/N_(Tot))λ_(tr) of λ_(tr) comes from <α²F₁>and the fraction (1−N_(4M)/N_(Tot))λ_(tr) comes from <α²F₂>leading to

$\begin{matrix} {\begin{matrix} {{{\lambda_{tr}\left( {1 - \frac{N_{4M}}{N_{Tot}}} \right)} = {2{\int}_{0}^{+ \infty}d\Omega\frac{\left\langle {\alpha^{2}{F_{2}\left( {k,k^{\prime},\Omega} \right)}} \right\rangle}{\Omega}}},} \\ {{\lambda_{tr} = {2C_{2}{\int}_{0}^{\omega_{D}}\frac{d\Omega}{\omega_{D}}}},} \\ {\lambda_{tr} = {2C_{2}}} \end{matrix},} & \left( {G36} \right) \end{matrix}$ $\begin{matrix} {\begin{matrix} {{{\lambda_{tr}\left( \frac{N_{4M}}{N_{Tot}} \right)} = {2{\int}_{\omega_{\min}}^{\omega_{D}}d\Omega\frac{\left\langle {\alpha^{2}{F_{1}\left( {k,k^{\prime},\Omega} \right)}} \right\rangle}{\Omega}}},} \\ {{\lambda_{tr} = {2C_{2}{\int}_{\omega_{\min}}^{\omega_{D}}\frac{d\Omega}{\Omega}}},} \\ {\lambda_{tr} = {C_{1}\left\lbrack {2{\ln\left( \frac{\omega_{D}}{\omega_{\min}} \right)}} \right\rbrack}} \end{matrix}.} & \left( {G37} \right) \end{matrix}$

Substituting C₁ and C₂ in terms of λ_(tr) back into α²F₁ and α²F₂ yields

$\begin{matrix} {{{\alpha^{2}{F_{1}\left( {k,k^{\prime},\Omega} \right)}} = {{\lambda_{tr}\left\lbrack {\ln\left( \frac{\omega_{D}}{\omega_{\min}} \right)}^{2} \right\rbrack}^{- 1}{D(k)}{D\left( k^{\prime} \right)}\left( \frac{N_{4M}}{N_{Tot}} \right)}},{\omega_{\min} < \Omega < \omega_{D}},} & \left( {G38} \right) \end{matrix}$ and $\begin{matrix} {{{\alpha^{2}{F_{2}\left( {k,k^{\prime},\Omega} \right)}} = {\frac{1}{2}{\lambda_{tr}\left( \frac{\Omega}{\omega_{D}} \right)}\left( {1 - \frac{N_{4M}}{N_{Tot}}} \right)}},{0 < \Omega < {\omega_{D}.}}} & \left( {G39} \right) \end{matrix}$

α²F₁=0 outside of the range ω_(min)<Ω<ω_(D) and α²F₂=0 for Ω>ω_(D).

We solve for λ(k, k′, ω_(n))or i=1, 2 using the k-space version of equation G4

$\begin{matrix} {{{\lambda_{i}\left( {k,k^{\prime},\omega_{n}} \right)} = {{\int}_{0}^{+ \infty}d{\Omega\alpha}^{2}{F_{i}\left( {k,k^{\prime},\Omega} \right)}\left( \frac{2\omega}{\omega_{n}^{2} + \Omega^{2}} \right)}},} & \left( {G40} \right) \end{matrix}$ leadingto $\begin{matrix} {{\lambda_{1}\left( {k,k^{\prime},\omega_{n}} \right)} = {\left( \frac{N_{4M}}{N_{Tot}} \right)\lambda_{tr}{D(k)}{{D\left( k^{\prime} \right)}\left\lbrack \frac{\ln\left( \frac{\omega_{n}^{2} + \omega_{D}^{2}}{\omega_{n}^{2} + \omega_{\min}^{2}} \right)}{\ln\left( \frac{\omega_{D}^{2}}{\omega_{\min}^{2}} \right)} \right\rbrack}}} & \left( {G41} \right) \end{matrix}$ and $\begin{matrix} {{\lambda_{2}\left( {k,k^{\prime},\omega_{n}} \right)} = {\left( {1 - \frac{N_{4M}}{N_{Tot}}} \right){\lambda_{tr}\left\lbrack {1 - {\frac{❘\omega_{n}❘}{\omega_{D}}{\tan^{- 1}\left( \frac{\omega_{D}}{❘\omega_{n}❘} \right)}}} \right\rbrack}}} & \left( {G42} \right) \end{matrix}$

4. Generalization of the Eliashberg Equations for Multi-Layer Cuprates

The Eliashberg equations G11, G12, and G13 for a single CuO₂ layer per unit cell are generalized to multi-layer cuprates by changing k and k′ to bk and b′k′, respectively, in the single layer Eliashberg equations.

$\begin{matrix} {{{Z\left( {{bk},{i\omega_{n}}} \right)} = {1 + {\frac{\pi T}{❘\omega_{n}❘}{\sum\limits_{b^{\prime}k^{\prime}n^{\prime}}^{{❘\omega_{n^{\prime}}❘} < \omega_{c}}{\left\lbrack \frac{\delta\left( {\epsilon_{b^{\prime}k^{\prime}} - \epsilon_{F}} \right)}{N(0)} \right\rbrack{\lambda\left( {{bk},{b^{\prime}k^{\prime}},{\omega_{n} - \omega_{n^{\prime}}}} \right)}s_{n}s_{n^{\prime}}}}}}},} & ({G43}) \end{matrix}$ ${{{Z\left( {{bk},{i\omega_{n}}} \right)}{\Delta\left( {{bk},{i\omega_{n}}} \right)}} = {\pi T \times {\sum\limits_{b^{\prime}k^{\prime}n^{\prime}}^{{❘\omega_{n^{\prime}}❘} < \omega_{c}}{{{\frac{1}{❘\omega_{n^{\prime}}❘}\left\lbrack \frac{\delta\left( {\epsilon_{b^{\prime}k^{\prime}} - \epsilon_{F}} \right)}{N(0)} \right\rbrack}\left\lbrack {{\lambda\left( {{bk},{b^{\prime}k^{\prime}},{\omega_{n} - \omega_{n^{\prime}}}} \right)} - {\mu^{*}\left( \omega_{c} \right)}} \right\rbrack}{\Delta\left( {{b^{\prime}k^{\prime}},{i\omega_{n^{\prime}}}} \right)}}}}},$ $\begin{matrix} {{{Z\left( {{bk},{{- i}\omega_{n}}} \right)} = {{Z\left( {{bk},{i\omega_{n}}} \right)} = {{Real}{Number}}}},} & ({G44}) \end{matrix}$ $\begin{matrix} {{{\Delta\left( {{bk},{{- i}\omega_{n}}} \right)} = {{\Delta\left( {{bk},{i\omega_{n}}} \right)} = {{Real}{Number}}}},} & ({G45}) \end{matrix}$

where b and b′ are band indicies. They vary from 1 to L, where L, is the number of CuO₂ layers per unit cell. A unit cell contains L Cu atoms, one in each layer. The k vector is a 21) vector. N(0) is the total density of states per spin

$\begin{matrix} {{N(0)} = {\sum\limits_{b^{\prime}k^{\prime}}{{\delta\left( {\epsilon_{b^{\prime}k^{\prime}} - \epsilon_{F}} \right)}.}}} & ({G46}) \end{matrix}$

There is a Bloch k state for each layer, l, given by ϕ(ik). The band eigenfunctions are

$\begin{matrix} {{\psi({bk})} = {\sum\limits_{i}{{A_{bl}(k)}{{\phi({lk})}.}}}} & ({G47}) \end{matrix}$

The coefficients, A_(bl)(k), are real since the inter-layer hopping matrix elements are real. The matrix element for hopping between adjacent layers is

<ϕ(l±1k′)|H _(inter)|ϕ(k)>=−t(l±1,l,k)δ,_(k′k)  (G48)

where

t(l±1,l,k)=αt_(z)(¼)[cos(k _(x) a)−cos(k

a)]²,  (G49)

and α is the product of the fraction of metallic sites in layers l and l±1. See Appendix F Table 11.

The eigenvectors Ψ(bk) of equations G47 and G48 are independent of the magnitude of t(l±1, l, k). Thus A_(bl)(k) is independent of k.

A _(bl)(k)=A _(bl).  (G50)

The eigenstates, Ψ(bk), are normalized leading to

$\begin{matrix} {{{\sum\limits_{b}{A_{{bl}^{\prime}}A_{bl}}} = \delta_{{ll}^{\prime}}},} & ({G51}) \end{matrix}$ $\begin{matrix} {{\sum\limits_{l}{A_{b^{\prime}l}A_{bl}}} = {\delta_{b^{\prime}b}.}} & ({G52}) \end{matrix}$

The electron-phonon spectral function α²F₂(bk, b′k′, Ω) is

$\begin{matrix} {{{\alpha^{2}{F_{2}\left( {{bk},{b^{\prime}k^{\prime}},\Omega} \right)}} = {\frac{1}{2}{\lambda_{tr}\left( \frac{\Omega}{\omega_{D}} \right)}\left( {1 - n_{4M}} \right)}},{0 < \Omega < \omega_{D}},} & ({G53}) \end{matrix}$ where $\begin{matrix} {{{n_{4m}(l)} = \frac{N_{4M}(l)}{N_{xy}}},} & ({G54}) \end{matrix}$ $\begin{matrix} {n_{4M} = {\frac{1}{L}{\sum\limits_{l}{{n_{4M}(l)}.}}}} & ({G55}) \end{matrix}$

N_(4M)(l) is the number of metallic Cu sites in layer l that are in non-overlapping plaquettes, L is the total number of CuO₂ layers per unit cell, and N_(x)

is the total number of Cu sites (metallic plus insulating AF) in a single CuO₂ layer. Hence, LN_(x)

is the total number of Cu sites in the crystal and n_(4M) is the total fraction of metallic Cu sites over all the CuO₂ layers, α²F₂=0 for Ω>ω_(D).

For the electron-phonon spectral function, α²F₁, that leads to the low-temperature linear resistivity, define the anisotropy factor, D(bk) as

$\begin{matrix} {{D({bk})} = \frac{\left( {{\cos\left( {k_{x}a} \right)} - {\cos\left( {k_{y}a} \right)}} \right)^{2}}{\left\langle \left( {{\cos\left( {k_{x}a} \right)} - {\cos\left( {k_{y}a} \right)}} \right)^{2} \right\rangle}} & ({G56}) \end{matrix}$

where the denominator is the average over all the L Fermi surface-s of the numerator.

The average of a function, f(bk), over all the Fermi surfaces is defined as

$\begin{matrix} {\left\langle {f({bk})} \right\rangle = {\frac{{{\sum}_{b^{\prime}k^{\prime}}\left\lbrack \frac{\delta\left( {\epsilon_{b^{\prime}k^{\prime}} - \epsilon_{F}} \right)}{N(0)} \right\rbrack}{f\left( {b^{\prime}k^{\prime}} \right)}}{{\sum}_{b^{\prime}k^{\prime}}\left\lbrack \frac{\delta\left( {\epsilon_{b^{\prime}k^{\prime}} - \epsilon_{F}} \right)}{N(0)} \right\rbrack}.}} & ({G57}) \end{matrix}$

The phonon modes in α²F₁ are 2D. Hence the form of the spectral function between layers l and l′ is of the form,

$\begin{matrix} {{\alpha^{2}{F_{1}\left( {{lk},{l^{\prime}k^{\prime}},\Omega} \right)}} = {{\delta_{{ll}^{\prime}}\left\lbrack {\ln\left( \frac{\omega_{D}^{2}}{\omega_{\min}^{2}} \right)} \right\rbrack}^{- 1}{n_{4m}(l)}{D(k)}{{D\left( k^{\prime} \right)}.}}} & ({G58}) \end{matrix}$

Expanding the eigenstates Ψ(bk) in terms of ϕ(k) from equation G47 leads to

Where ω_(min)<Ω<ω_(D). α²F₁=0, for Ω<ω_(min)or Ω>ω_(D).

Hence,

$\begin{matrix} {{{\alpha^{2}{F_{1}\left( {{bk},{b^{\prime}k^{\prime}},\Omega} \right)}} = {\left\{ {\sum\limits_{l}{{❘A_{bl}❘}^{2}{❘A_{b^{\prime}l^{\prime}}❘}^{2}{n_{4m}(l)}}} \right\}{\lambda_{tr}\left\lbrack {\ln\left( \frac{\omega_{D}^{2}}{\omega_{\min}^{2}} \right)} \right\rbrack}^{- 1}{D({bk})}{D\left( {b^{\prime}k^{\prime}} \right)}}},} & ({G59}) \end{matrix}$

$\begin{matrix} {{\lambda_{1}\left( {{bk},{b^{\prime}k^{\prime}},\omega_{n}} \right)} = {\left\{ {\sum\limits_{l}{{❘A_{bl}❘}^{2}{❘A_{b^{\prime}l^{\prime}}❘}^{2}{n_{4m}(l)}}} \right\}\lambda_{tr}{D({bk})}{{D\left( {bk}^{\prime} \right)}\left\lbrack \frac{\ln\left( \frac{\omega_{n}^{2} + \omega_{D}^{2}}{\omega_{n}^{2} + \omega_{\min}^{2}} \right.}{\ln\left( \frac{\omega_{D}^{2}}{\omega_{\min}^{2}} \right)} \right\rbrack}}} & ({G60}) \end{matrix}$ and $\begin{matrix} {\left. {{\lambda_{2}9{bk}},{b^{\prime}k^{\prime}},\omega_{n}} \right) = {\left( {1 - n_{4M}} \right){\lambda_{tr}\left\lbrack {1 - {\frac{❘\omega_{n}❘}{\omega_{D}}{\tan^{- 1}\left( \frac{\omega_{D}}{❘\omega_{n}❘} \right)}}} \right\rbrack}}} & ({G61}) \end{matrix}$

The multi-layer expressions for λ_(surf)(bk, b′k′, ω_(n)) and λ⊥(bk, b′k′, ω_(n)) are similar to their single-layer counterparts with a modified definition for the averaging in their respective J^((x)) and J^((y)) functions.

$\begin{matrix} {{{J_{surf}^{(x)}\left( {{bk},{b^{\prime}k^{\prime}}} \right)} = {{\left\langle \left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)^{2} \right\rangle_{x}\cos^{2}\frac{1}{2}\left( {k_{x}^{\prime} - k_{x}} \right)a} - {2\left\langle {\delta{t\left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)}} \right\rangle_{x}\cos\frac{1}{2}\left( {k_{x}^{\prime} - k_{x}} \right)a\cos\frac{1}{2}\left( {k_{x}^{\prime} + k_{x}} \right)a} + {{\left\langle {\delta t^{2}} \right\rangle_{x} \cdot 4}\cos^{2}\frac{1}{2}\left( {k_{x}^{\prime} + k_{x}} \right)a} + {\left\langle \left( {{\delta\epsilon}_{L} - {\delta\epsilon}_{R}} \right)^{2} \right\rangle_{x}\sin^{2}\frac{1}{2}\left( {k_{x}^{\prime} - k_{x}} \right)a}}},} & ({G62}) \end{matrix}$ $\begin{matrix} {{{J_{surf}^{(y)}\left( {{bk},{b^{\prime}k^{\prime}}} \right)} = {{\left\langle \left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)^{2} \right\rangle_{y}\cos^{2}\frac{1}{2}\left( {k_{y}^{\prime} - k_{y}} \right)a} - {2\left\langle {\delta{t\left( {{\delta\epsilon}_{L} + {\delta\epsilon}_{R}} \right)}} \right\rangle_{y}\cos\frac{1}{2}\left( {k_{y}^{\prime} - k_{y}} \right)a\cos\frac{1}{2}\left( {k_{y}^{\prime} + k_{y}} \right)a} + {{\left\langle {\delta t^{2}} \right\rangle_{y} \cdot 4}\cos^{2}\frac{1}{2}\left( {k_{y}^{\prime} + k_{y}} \right)a} + {\left\langle \left( {{\delta\epsilon}_{L} - {\delta\epsilon}_{R}} \right)^{2} \right\rangle_{y}\sin^{2}\frac{1}{2}\left( {k_{y}^{\prime} - k_{y}} \right)a}}},} & ({G63}) \end{matrix}$

where <F(R_(σ))>_(x) is the multi-layer average of the function F(R_(σ)) defined for each planar surface O on the x-axis with position R_(σ) as shown in FIG. 27 ,

$\begin{matrix} {{\left\langle {F\left( R_{\sigma} \right)} \right\rangle = {\sum\limits_{l}{{❘A_{bl}❘}^{2}{❘A_{b^{\prime}l^{\prime}}❘}^{2}\left\langle {F_{l}\left( R_{\sigma} \right)} \right\rangle}}},} & ({G64}) \end{matrix}$

and <F₁(R_(σ))>_(x) is the average over layer l, as defined in equation G21. Similarly for <F(R_(σ))>

. The expression in equation G63 for

is identical to the expression for J_(surf) ^((x)) in equation G62 with x replaced by y. Hence, λ_(surf)(bk, b′k′, ω_(n)) is

$\begin{matrix} {{{\lambda_{surf}\left( {k,k^{\prime},\omega_{n}} \right)} = {{\left( \frac{N(0)}{N_{M}} \right)\left\lbrack {{J_{surf}^{(x)}\left( {k,k^{\prime}} \right)} + {J_{surf}^{(y)}\left( {k,k^{\prime}} \right)}} \right\rbrack}\left( \frac{2\omega_{ph}}{\omega_{n}^{2} + \omega_{ph}^{2}} \right)}},} & ({G65}) \end{matrix}$

where N_(M) is the total number of metallic Cu sites N_(M)=Σ₁N_(1M), and N_(1M) is the total number of metallic Cu sites In layer l.

For λ⊥(bk, b′k′, ω_(n)), the corresponding J_(⊥) ^((x)) and

functions are

J _(⊥) ^((x))(bk,b′k′)=

δ∈²

_(x)−2

δ∈[δt(+)+δf(−)]

_(x)(cos k′ _(x) a+cos k _(x) a)

+

[δt(+)+δt(−)]

_(x)(cos k _(x) ^(J) a+cos k _(x) a)²

+

[δt(+)−δt(−)]

_(x)(sin k _(x) ^(J) a−sin k _(x) a)²  (G66)

J _(⊥) ^((y))(bk,b′k′)=

δ∈²

_(y)−2 (δ∈[δt(+)+δt(−)]

_(y)(cos k′ _(y) a+cos k _(y) a)

+

[δt(+)+δt(−)]

_(y)(cos k′ _(y) a+cos k _(y) a)²

+

[δt(+)−δt(−)]

_(y)(sin k′ _(y) a−sin k _(y) a)²  (G67)

All averages in equations G66 and G67 are defined in equation G64.

Hence λ_(⊥)(bk, b′k′, ω_(n)) is

$\begin{matrix} {{\lambda_{\bot}\left( {{bk},{b^{\prime}k^{\prime}},\omega_{n}} \right)} = {{\left( \frac{N(0)}{N_{M}} \right)\left\lbrack {{J_{\bot}^{(x)}\left( {{bk},{b^{\prime}k^{\prime}}} \right)} + {J_{\bot}^{(y)}\left( {{bk},{b^{\prime}k^{\prime}}} \right)}} \right\rbrack}{\left( \frac{2\omega_{ph}}{\omega_{n}^{2} + \omega_{ph}^{2}} \right).}}} & ({G68}) \end{matrix}$

5. Computational Details

The band structure, ∈_(k), and all the parameters used the solve the Eliashberg equations for T_(c) are described in Appendix F. Here, we discuss the computational issues necessary to obtain an accurate T_(c).

The two planar interface O atom phonon modes in FIG. 12 require averaging products of pairs of parameters (δ∈_(L), δ∈_(R), and δt for λ_(surf), and δ∈ and δt(±) for λ_(⊥)) over the lattice as seen in equations G19, G20, G26, G27, G62, G63 G66 and G07. These parameters vary depending on the environment of the Cu atoms, as shown in FIG. 12 .

For each doping value, we generate a 2000×2000 lattice of doped plaquettes. All O atoms that contribute to λ_(surf) and λ_(⊥) are identified along with the nature of the corresponding Cu sites (edge, convex, or concave, as shown in FIG. 12 ). All the product averages are computed. Ensembles of 2000×2000 lattices can be generated to obtain more accurate product averages. We found that a single 2000×2000 doped lattice is large enough to obtain all the products to an accuracy of less than 1%.

All four electron-phonon pairing functions, λ₁, λ₂, λ_(surf), and λ_(⊥) can be written in the following product form λ(k, k′, ω_(n))=λ′(k k′)F(ω_(n)). The product separation, λ=λ′F, leads to a large reduction in the storage requirements because λ′ and F can be computed once and saved, and the product computed on the fly.

We discretize the Fermi surface by choosing 10 uniformly spaced (in angle) k-points in the 45° wedge bounded by the vectors along the x-axis, (π, 0), and the diagonal, (π, π), leading to a total of 80 k-points over the full Fermi surface. Increasing the number of k-points further led to <0.1 K change in the calculated T_(c).

Fermi surface weights, W_(bk), are computed at each bk-point using the Fermi velocity evaluated from the band structure, ∈_(k). By rescaling the gap function, Δ(bk, ω_(n)),

$\begin{matrix} {{\Delta^{\prime}\left( {{bk},\omega_{n}} \right)} = {\left\lbrack \frac{W_{bk}}{❘{{2n} + 1}❘} \right\rbrack^{\frac{1}{2}}{\Delta\left( {{bk},\omega_{n}} \right)}}} & ({G69}) \end{matrix}$

the Eliashberg equations can be turned into an eigenvalue equation with a real symmetric matrix.¹⁶ Since T_(c) occurs when the largest eigenvalue reaches one, we can perform a Lanczos projection. We compute T_(c) by bracketing. All the T_(c) values found in this paper are accurate to ±0.3K. For approximate timings, a, full T_(c)-dome is computed on a small workstation in ≈5-10 minutes.

Advantages and Improvements

Presented herein is a method of fabricating high temperature superconductors. The validity of the method is illustrated using a microscopic theory of cuprate superconductivity based on the results of the chemist's ab initio hybrid density functional methods (DFT). Hybrid DFT finds a localized out-of-the-CuO₂ hole is formed around a negatively charged dopant. The doped hole resides in a four-Cu-site plaquette. The out-of-plane hole destroys the antiferromagnetism inside the plaquette and creates a tiny piece of metal there. Hence, the crystal is inhomogeneous on the atomic-scale with metallic and insulating regions.

In contrast, the physicist's DFT methods (LDA and PBE) find a delocalized hole residing in the CuO₂ planes as a consequence of doping. As discussed herein, the chemist's result is to be trusted over the physicist's result because it corrects the spurious self-Coulomb repulsion of the electrons found in the physicist's density functionals.

Due to dopant-dopant Coulomb repulsion, doped plaquettes do not overlap unless the doping is sufficiently high that overlap cannot be avoided. Non-overlapping plaquettes have a dynamic Jahn-Teller distortion of the out-of-the-plane hole (called a “fluctuating dumbbell”). The dumbbells inside an overlapped plaquette become static Jahn-Teller distor-tions, or “frozen”.

The above model explains a vast swath of normal state phenomenology using simple counting of the sizes of the metallic region, the insulating AF region, and the number of fluctuating and frozen dumbbells. As illustrated herein, superconducting pairing arises from planar Oxygen atoms near the interface between the metallic and insulating regions. These planar O atom phonon modes explain the large T_(c)˜100 K, the Tc-dome as a function of doping, the changes in Tc as a function of the number of CuO₂ layers per unit cell, the lack of a Tc isotope effect at optimal doping, and the D-wave superconducting pairing wavefunction (or superconducting gap symmetry).

Generally, with phonon superconducting pairing, an isotropic S-wave pairing wavefunction is favored over a D-wave pairing wavefunction. However, the present disclosure shows that the fluctuating dumbbells drastically raise the Cooper pair Coulomb repulsion, leading to the observed D-wave pairing wavefunction. By overlapping the plaquettes and freezing the dumbbells, the S-wave pairing wavefunction becomes favored over the D-wave pairing wavefunction. The present disclosure shows that the S-wave Tc is in the range of ≈280-390 K when the D-wave Tc≈100 K.

REFERENCES

The following references are incorporated by reference herein.

-   1 Schilling, A., Cantoni, M., Guo, J. D. & Ott, H. R.     Superconductivity above 130 k in the Hg—Ba—Ca—Cu-o system. Nature     363, 56-58 (1993). -   2 Mukuda, H., Shimizu, S., Iyo, A. & Kitaoka, Y. High-tc     superconductivity and antiferromagnetism in multilayered copper     oxides-a new paradigm of superconducting mechanism. Journal of the     Physical Society of Japan 81, 011008 (2012). -   3 Mann, A. Still in suspense. Nature 475, 280-282 (2011). -   4 Perdew, J. P., Burke, K. & Emzerhof, M. Generalized gradient     approximation made simple. Phys. Rev. Lett. 77, 3865-3868 (1996).     URL http://link.aps.org/doi/10.1103/PhysRevLett.77.3865. -   5 Yu, J. J., Freeman, A. J. & Xu, J. H. Electronically driven     instabilities and superconductivity in the layered     La_(2-x)Ba_(x)CuO₄ perovskites. Physical Review Letters 58,     1035-1037 (1987). -   6 Mattheiss, L. F. Electronic band properties and superconductivity     in 1a2-yxycuo4. Physical Review Letters 58, 1028-1030 (1987). -   7 Pickett, W. E. Electronic-structure of the high-temperature oxide     superconductors. Reviews of Modern Physics 61, 433-512 (1989). -   8 Perdew, J. P. & Zunger, A. Self-interaction correction to     density-functional approximations for many-electron systems.     Physical Review B 23, 5048-5079 (1981). -   9 Perry, J. K., Tahir-Kheli, J. & Goddard, W. A. Antiferromagnetic     band structure of 1a2cuo4: Becke-3-lee-yang-parr calculations.     Physical Review B 63, 144510 (2001). -   10 Perry, J. K., Tahir-Kheli, J. & Goddard, W. A. Ab initio evidence     for the formation of impurity d3z2-r2 holes in doped 1a2-xsrxcuo4.     Physical Review B 65, 144501 (2002). -   11 Tahir-Kheli, J. & Goddard, W. A. Origin of the pseudogap in     high-temperature cuprate superconductors. Journal of Physical     Chemistry Letters 2, 2326 2330 (2011). -   12 Tahir-Kheli, J. Understanding superconductivity in cuprates.     Caltech YouTuhe Channel (2015). URL     https://wwwv.youtube.com/watch?v=Dg2u1zS U9k. -   13 Tahir-Kheli, J. Resistance of high-temperature cuprate     superconductors. New Journal of Physics 15, 073020 (2013). -   14 Tahir-Kheli, J. & Goddard, W. A. Universal properties of cuprate     superconductors: Tc phase diagram, room-temperature thermopower,     neutron spin resonance, and sun incommensurability explained in     terms of chiral plaquette pairing. Journal of Physical Chemistry     Letters 1, 1290-1295 (2010). -   15 Proust, C., Vignolle, B., Levallois, J., Adachi, S. &     Hussey, N. E. Fermi liquid behavior of the in-plane resistivity in     the pseudogap state of yba2cu4o8. Proceedings of the National     Academy of Sciences 113, 13654-13659 (2016). URL     http://www.pnas.org/content/113/48/13654. abstract.     http://www.pnas.org/content/113/48/13654.full.pdf. -   16 Allen, P. B. & Mitrovic, B. Theory of superconducting tc. In     Ehrenreich, H., Seitz, F. & Turnbull, D. (eds.) Solid State Physics,     Advances in Research and Applications, vol. 37, 1-92 (Academic     Press, New York, 1982). -   17 Hashimoto, M. et al. Doping evolution of the electronic structure     in the single-layer cuprate bi2sr2-xlaxCuo6+6: Comparison with other     single-layer cuprates. Phys. Rev. B 77, 094516 (2008). URL     http://link.aps.org/doi/10.1103/PhysRevB. 77.094516. -   18 Pintschovius, L. Electron-phonon coupling effects explored by     inelastic neutron scattering. Physcaa Status Solidi B-Basic Research     242, 30-50 (2005). -   19 Phillips, J. C. Self-organized networks and lattice effects in     high-temperature superconductors. Physical Review B 75 (2007). -   20 Li, C. W. et al. Structural relationship between negative thermal     expansion and quartic anharmonicity of cubic scf3. Phys. Rev. Lett.     107, 195504 (2011). URL     http://link.aps.org/doi/10.1103/PhysRevLett.107.195504. -   21 Lan, T. et al. Anharmonic lattice dynamics of Ag2O studied by     inelastic neutron scattering and first-principles molecular dynamics     simulations. Phys. Rev. B 89, 054306 (2014). URL     http://link.aps.org/doi/10.1103/PhysRevB.89.054306. -   22 Hui, J. C. K. & Allen, P. B. Effect of lattice anharmonicity on     superconductivity. Journal of Physics F: Metal Physics 4, L42     (1974). URL http://stacks.iop.org/0305-4608/4/i=3/a=003. -   23 Crespi, V. H., Cohen, M. L. & Penn, D. R. Anharmonic phonons and     the isotope effect in superconductivity. Phys. Rev. B 43,     12921-12924 (1991). URL     http://link.aps.org/doi/10.1103/PhysRevB.43.12921. -   24 Crespi, V. H. & Cohen, M. L. Anharmonic phonons and the anomalous     isotope effect in lag-x srx cuo4. Phys. Rev. B 44, 4712-4715 (1991).     URL http://link.aps.org/doi/10.1103/PhysRevB.44.4712. -   25 Crespi, V. H. & Cohen, M. L. Anharmonic phonons and     high-temperature superconductivity. Phys. Rev. B 48, 398-406 (1993).     URL http://link.aps.org/doi/10.1103/PhysRevB.48. 398. -   26 Keller, H. Unconventional isotope effects in cuprate     superconductors. In Müller, K. A. & Bussmann-Holder, A. (eds.) In     Superconductivity in Complex Systems. Springer Series Structure and     Bonding, vol. 114, 143-169 (Springer Berlin Heidelberg, Berlin,     Heidelberg, 2005). URL http://dx.doi.org/10.1007/b101019. -   27 Keller, H., Bussmann-Holder, A. & Miler, K. A. Jahnteller physics     and high-tc superconductivity. Materials Today 11, 38-46 (2008).     URL//www.sciencedirect.com/scicnce/article/pii/S 1369702108701780. -   28 de Gennes, P. G. Superconductivity of Metals and Alloys     (Addison-Wesley Publishing Co., Inc., Redwood City, California,     1989). -   29 Schreiffer, J. R. Theory of Superconductivity (Perseus Books,     Reading, Massachusetts, 1999). -   30 Bogoliubov, N. N., Tolamachev, V. V. & Shirkov, D. V. A New     Method in the Theory of Superconductivity (Consultants Bureau, Inc.,     New York, 1959). -   31 Morel, P. & Anderson, P. W. Calculation of the superconducting     state parameters with retarded electron-phonon interaction. Phys.     Rev. 125, 1263-1271 (1962). URL     http://link.aps.org/doi/10.1103/PhysRev.125.1263. -   32 Cohen, M. L. Superconductivity in low-carrier density systems:     Degenerate semiconductors. In Parks, R. D. (ed.) Superconductivity,     vol. 1, 615-664 (Marcel Dekker, Inc., New York, 1969). -   33 Tsuei, C. C. & Kirtley, J. R. Pairing symmetry in cuprate     superconductors. Rev. Mod Phis. 72, 969-1016 (2000). URL     http://link.aps.org/doi/10.1103/RevModPhys.72.969. -   34 Schrieffer, J. R., Scalapino, D. J. & Wilkins, J. W. Effective     tunneling density of states in superconductors. Phys. Rev. Lett. 10,     336-339 (1963). URL     http://link.aps.org/doi/10.1103/PhysRevLett.10.336. -   35 Scalapino, D. J., Schrieffer, J. R. & Wilkins, J. W.     Strong-coupling superconductivity. i. Phys. Rev. 148, 263-279     (1966). URL http://link.aps.org/doi/10.1103/PhysRev.148.263. -   36 Karppinen, M. et al. Layer-specific hole concentrations in     bi2sr2y 1-xcax)cu208+6 as probed by xanes spectroscopy and     coulometric redox analysis. Phys. Rev. B 67, 134522 (2003). URL     http://link.aps.org/doi/10.1103/PhysRevB.67.134522. -   37 Liang, R., Bonn, D. A. & Hardy, W. N. Evaluation of cuo2 plane     hole doping in yba2cu3o6+x single crystals. Phys. Rev. B 73, 180505     (2006). URL http://link.aps.org/doi/10.1103/PhysRevB.73.180505. -   38 Naqib, S. H., Cooper, J. R., Tallon, J. L. & Panagopoulos, C.     Temperature dependence of electrical resistivity of high-t-c     cuprates—from pseudogap to overdoped regions. Physica     C-Superconductivity and Its Applications 387, 365-372 (2003). -   39 Yoshida, T. et al. Low-energy electronic structure of the high-tc     cuprates 1a2-xsrxcuo4 studied by angle-resolved photoemission     spectroscopy. Journal of Physics: Condensed Matter 19, 125209(2007).     URL http://stacks.iop.org/0953-8984/19/i=12/a=125209. -   40 Ono, S. & Ando, Y. Evolution of the resistivity anisotropy in     bi2sr2-xlaxcuo6+8 single crystals for a wide range of hole doping.     Phys. Rev. B 67, 104512 (2003). URL     http://link.aps.org/doi/10.1103/PhysRevB.67.104512. -   41 Bangura, A. F. et al. Fermi surface and electronic homogeneity of     the overdoped cuprate superconductor t12ba2cuo6+S as revealed by     quantum oscillations. Phys. Rev. B 82, 140501(2010). URL     http://link.aps.org/doi/10.1103/PhysRevB.82 0.140501. -   42 Rourke, P. M. C. et al. A detailed de haasvan alphen effect study     of the overdoped cuprate t12ba2cuo6+8. New Journal of Physics 12,     105009 (2010). URL http://stacks.iop.org/1367-2630/12/i=10/a=105009. -   43 Kurtin, S., McGill, T. C. & Mead, C. A. Fundamental transition in     the electronic nature of solids. Phys. Rev. Lett. 22, 1433-1436     (1969). URL htqx//link.aps.org/doi/10.1103/PhysRevLett.22.1433. -   44 Takagi, H. et al. Superconductor-to-nonsuperconductor transition     in (lal-xsrx)2cuo4 as investigated by transport and magnetic     measurements. Phys. Rev. B 40, 2254-2261 (1989). URL     http://link.aps.org/doi/10.1103/PhysRevB.40.2254. -   45 Herzberg, G. Molecular Spectra and Molecular Structure I. Spectra     of Diatomic Molecules (D. Van Nostrand Company, Inc. Princeton, New     Jersey, 1950). -   46 Herzberg, G. Molecular Spectra and Molecular Structure II.     Infrared and Raman Spectra of Polyatomic Molecules (D. Van Nostrand     Company, Inc. Princeton, New Jersey, 1945). -   47 Wilson, E. B., Decius, J. C. & Cross, P. C. Molecular Vibrations.     The Theory of Infrared and Raman Vibrational Spectra (Dover     Publications, Inc., New York, 1980). -   48 Pereiro, J. et al. Insights from the study of high-temperature     interface superconductivity. Philosophical Transactions of the Royal     Society of London A: Mathematical. Physical and Engineering Sciences     370, 4890-4903 (2012). URL     http://rsta.royalsocietypublishing.org/content/370/1977/4890.     http://rsta. royal soci etypu bl ishing.org/content/370/1977/4890.     full .pdf. -   49 Allen, P. B. & Dynes, R. C. Transition temperature of     strong-coupled superconductors reanalyzed. Phys. Rev. B 12, 905-922     (1975). URL http://link.aps.org/doi/10.1103/PhysRevB.12.905. -   50 Blatt, J. M. Theory of Superconductivity (Academic Press Inc.,     New York and London, 1964). -   51 Crowley, J. M., Tahir-Kheli, J. & Goddard, W. A. Resolution of     the band gap prediction problem for materials design. J. Phys. Chem.     Lett. 7, 1198-1203 (2016). URL http://dx.doi.     org/10.1021/acs.jpclett.5b02870.     http://dx.doi.org/10.1021/acs.jpclett.5b02870. -   52 Ginder, J. M. et al. Photoexcitations in 1a2cuo4: 2-ev energy gap     and long-lived defect states. Phys. Rev. B 37, 7506-7509 (1988). -   53 Zhang, F. C. & Rice, T. M. Effective hamiltonian for the     superconducting cu oxides. Phys. Rev. B 37, 3759-3761 (1988). URL     http://link.aps.org/doi/10.1103/PhysRevB.37.3759. -   54 Becke, A. D. Density-functional thermochemistry. iii. the role of     exact exchange. J. Chem. Phys. 98, 5648-5652 (1993). URL     http://scitation.aip.org/content/aip/joumal/jcp/98/7/10.1063/1.464913.     55 Saunders, V. et al. CRYSTAL98 User's Manual (University of     Torino: Torino, 1998). -   56 Lee, C., Yang. W. & Parr, R. G. Development of the colle-salvetti     correlation-energy formula into a functional of the electron     density. Phys. Rev. B 37, 785-789 (1988). URL http://link.     aps.org/doi/10.1103/PhysRevB.37.785. -   57 CRYSTAL98 only had basic Fock Matrix mixing convergence (SCF) at     the time of our calculation in 2001.[9] Using the most recent     version of CRYSTAL (2015), we find the gap to be 3.1 eV using     exactly the same basis set. Improved SCF convergence algorithms,     increased computing power, and memory indicates our result of 2001     had not fully converged. We know hybrid functionals generally     overestimate the band gaps of Mott antiferromagnets by≈1 eV,[51]     perhaps because the unrestricted spin wavefunctions (UHF) do not     represent the correct spin state. Regardless, the orbital character     of the doped hole is unchanged. None of the conclusions of the     current disclosure are altered. -   58 Hybertsen, M. S., Stechel, E. B., Foulkes, W. M. C. &     Schluter, M. Model for low-energy electronic states probed by x-ray     absorption in high-tc cuprates. Physical Review B 45, 10032-10050     (1992). -   59 Scalapino, D. J. The electron-phonon interaction and     strong-coupling superconductors. In Parks, R. D. (ed.)     Superconductivity, vol. 1, 449-560 (Marcel Dekker, Inc., New York,     1969). -   60 Vidberg, H. J. & Serene, J. W. Solving the eliashberg equations     by means of n-point pad'e approximants. Journal of Low Temperature     Physics 29, 179-192 (1977). URL http://dx.doi.     org/10.1007/BF00655090. -   61 Leavens, C. & Ritchie, D. Extension of the n-point pad'e     approximants solution of the eliashberg equations to t˜tc. Solid     State Communications 53, 137-142 (1985).     URL//www.sciencedirect.com/science/article/pii/0038109885901127. -   62 Beach, K. S. D., Gooding, R. J. & Marsiglio, F. Reliable pad'e     analytical continuation method based on a high-accuracy symbolic     computation algorithm. Phys. Rev. B 61, 5147-5157 (2000). URL     http://link.aps.org/doi/10.1103/PhysRevB.61.5147. -   63 “Ostlin, A., Chioncel, L. & Vitos. L. One-particle spectral     function and analytic continuation for many-body implementation in     the exact muffin-tin orbitals method. Phys. Rev. B 86, 235107     (2012). URL http://link.aps.org/doi/10.1103/PhysRev B.86.235107. -   64 Elliott, R. J., krumhansl, J. A. & Leath, P. L. The theory and     properties of randomly disordered crystals and related physical     systems. Rev. Mod. Phys. 46, 465 543 (1974). URL http://link.     aps.org/doi/10.1103/RevModPhys.46.465. -   65 Hussey, N. E. et al. Dichotomy in the t-linear resistivity in     hole-doped cuprates. Philosophical Transactions of the Royal Society     a-Mathematical Physical and Engineering Sciences 369, 1626- -   66 Abdel-Jawad, M. et al. Anisotropic scattering and anomalous     normal-state transport in a high temperature superconductor. Nature     Physics 2, 821-825 (2006). -   67 Cooper, R. A. et al. Anomalous criticality in the electrical     resistivity of 1a2-xsrxcuo4. Science 323, 603-607 (2009).

CONCLUSION

This concludes the description of the preferred embodiment of the present invention. The foregoing description of one or more embodiments of the invention has been presented for the purposes of illustration and description. It is not intended to be exhaustive or to limit the invention to the precise form disclosed. Many modifications and variations are possible in light of the above teaching. It is intended that the scope of the invention be limited not by this detailed description, but rather by the claims appended hereto. 

1.-20. (canceled)
 21. A cuprate superconductor, comprising: a wire comprising: grain boundaries; an aperiodic lattice of CuO₂ planes; and first atoms occupying sites between said CuO₂ planes, dopant atoms comprising second atoms and third atoms occupying first atom sites, where the second atoms are p-type dopants relative to the first atoms, and the third atoms are n-type dopants relative to the first atoms; wherein: the total concentration of said dopant atoms is greater than 20% of the concentration of said first atoms, the concentration of said second atoms is greater than 5% of the concentration of said first atoms, and the concentration of said third atoms is greater than 5% of the concentration of said first atoms.
 22. The cuprate superconductor of claim 21, wherein the wire is configured to utilize an S-wave property of the cuprate superconductor.
 23. The cuprate superconductor of claim 21, characterized as an S-wave superconductor.
 24. The cuprate superconductor of claim 21, wherein the doping has increased the superconducting transition temperature relative to the undoped D-wave superconducting temperature.
 25. An electrical machine or power transmission device comprising the cuprate superconductor of claim 21, wherein: the electrical machine generates a magnetic flux in response to a current density flowing in the wire, and the electrical machine or the power transmission device is configured to utilize an S-wave property of the cuprate superconductor.
 26. A machine comprising the cuprate superconductor of claim
 24. 27. The cuprate superconductor of claim 21, wherein the first atoms have oxidation state plus three, the second atoms have oxidation state plus two, and the third atoms have oxidation state plus four.
 28. The cuprate superconductor of claim 27, wherein the first atoms comprise Yttrium or Lanthanum and the second atoms comprise Magnesium, Calcium, Strontium, Barium, Zinc, Cadmium, Copper, Nickel, or Cobalt, and wherein the third atoms comprise Titanium, Zirconium, Hafnium, Cerium, Carbon, Silicon, Germanium, Tin, or Lead.
 29. The cuprate superconductor of claim 21, wherein the third atoms comprise Cerium.
 30. The cuprate superconductor of claim 21, wherein the first atoms have oxidation state plus two, the second atoms have oxidation state plus one, the third atoms have oxidation state plus three.
 31. The cuprate superconductor of claim 30, wherein the first atoms comprise Magnesium, Calcium, Strontium, Barium, Zinc, Cadmium, Copper, Nickel, or Cobalt.
 32. The cuprate superconductor of claim 21, wherein the first atoms comprise Oxygen and the third atoms comprise Fluorine.
 33. A method of making a cuprate superconductor, comprising: fabricating a wire comprising: grain boundaries; an aperiodic lattice of CuO₂ planes; and first atoms occupying sites between said CuO₂ planes, dopant atoms comprising second atoms and third atoms occupying first atom sites, where the second atoms are p-type dopants relative to the first atoms, and the third atoms are n-type dopants relative to the first atoms; wherein: the total concentration of said dopant atoms is greater than 20% of the concentration of said first atoms, the concentration of said second atoms is greater than 5% of the concentration of said first atoms, and the concentration of said third atoms is greater than 5% of the concentration of said first atoms; and measuring an S-wave property of the cuprate superconductor.
 34. The method of claim 33, wherein: the first atoms comprise Yttrium or Lanthanum and the second atoms comprise Magnesium, Calcium, Strontium, Barium, Zinc, Cadmium, Copper, Nickel, or Cobalt, and wherein the third atoms comprise Titanium, Zirconium, Hafnium, Cerium, Carbon, Silicon, Germanium, Tin, or Lead.
 35. The method of claim 33, wherein the third atoms comprise Cerium.
 36. The method of claim 33, wherein: the first atoms have oxidation state plus two, the second atoms have oxidation state plus one, the third atoms have oxidation state plus three, or the first atoms have oxidation state plus three, the second atoms have oxidation state plus two, and the third atoms have oxidation state plus four.
 37. The method of claim 33, further comprising: fabricating an electrical machine or power transmission device comprising the cuprate superconductor of claim 33, wherein: the electrical machine generates a magnetic flux in response to a current density flowing in the wire, and the electrical machine or the power transmission device is configured to utilize an S-wave property of the cuprate superconductor.
 38. The method of claim 37, wherein the doping has increased the superconducting transition temperature relative to the undoped D-wave superconducting temperature.
 39. A method of using a cuprate superconductor, comprising: obtaining a wire comprising: grain boundaries; an aperiodic lattice of CuO₂ planes; and first atoms occupying sites between said CuO₂ planes, dopant atoms comprising second atoms and third atoms occupying first atom sites, where the second atoms are p-type dopants relative to the first atoms, and the third atoms are n-type dopants relative to the first atoms; wherein: the total concentration of said dopant atoms is greater than 20% of the concentration of said first atoms, the concentration of said second atoms is greater than 5% of the concentration of said first atoms, and the concentration of said third atoms is greater than 5% of the concentration of said first atoms; and using an S-wave property of the cuprate superconductor.
 40. The method of claim 39, wherein using the S-wave property comprises using a stability against the grain boundaries. 